Fatigue Thesis
Short Description
fatigue thesis full...
Description
Fatigue Assessment of Components Subjected to NonProportional Stress Histories
Øyvind Aleksander Bruun
Master of Science in Mechanical Engineering Submission date: December 2013 Supervisor: Gunnar Härkegård, IPM Cosupervisor: Bjørn Haugen, IPM
Norwegian University of Science and Technology Department of Engineering Design and Materials
THE NOR WEGIAN UNIVERSITY OF’ SCIENCE ANI) TECHNOLOGY DEPARTMENT OF’ ENG[NEERING DESIGN AND MATERIALS
MASTER THESIS AUTUMN 2013 FOR STUD.TECIIN. 0YVIND A. BRUUN
FATiGUE ASSESSMENT OF COMPONENTS SUBJECTED TO NONPROPORTIONAL STRESS HISTORLES Utmattingsvurd ering av kom ponenter utsatte for ikkeproporsjonale spenningshistorier Traditional S—N based fatigue assessment criteria focus on uniaxial, constant amplitude loading. These criteria may be extended to multiaxial, variableamplitude stress histories under proportional loading by introducing an equivalent’ stress, such as the maximum principal stress amplitude or the von Mises stress amplitude (Sines, Crossland), together with suitable cyclecounting rules. The complexity of fatigue assessment is considerably in creased, if nonproportional stress histories are considered. Although several criticalplane’ theories (Findley, Dang Van. Matake, McDiarmid) have been proposed and implemented in FEA postprocessors for fatigue assessment of components under arbitrary multiaxial stress histories, these theories are still not well established in engineering design. When it comes to fatigue assessment based on fatiguecrack growth (FCG) in components under arbitrary multiaxial stress histories, the situation is even more unsatisfactory. Again most criteria and analytical tools assume uniaxial, constant amplitude loading. For multiaxial variable amplitude stress histories under proportional loading, crack growth is often assumed to he controlled by the maximum principal stress cycle. In a preceding project work ([lruun, 2013), a critical assessment was carried out of’ normal— stress modified’ shearstress based criticalplane models (due to Findley and Sines) and a maximumprincipalstress based criticalplane type model (due to I lempelMorrow) for the fatigue limit of a thin—walled tube under non—proportional normal—stress and shearstress
histories. The objective of this master assignment is to extend the project work to a broader set of models For the Fatigue assessment ot components subjected to non—proportional stress histories. The work should include S—N as well as FCG based criteria, applied to critical—load prediction for stress—histories below the fatigue limit and to Fatigue—life prediction For stresshistories above the ftitigue limit. In the latter case, suitable cycle—counting rules are to be discussed. Whenever possible. theoretical predictions should he compared with observations from fatigue testing.
The thesis should be written as a scientific report including • the (signed) project assignment, • a summary of the work (in English and Norwegian), • a table of contents, • the inducement and purpose of the assignment, • a presentation, demonstration and critical assessment of methods, • results, conclusions and recommendations, and • literature references. Figures and tables (including captions) should be largely selfexplanatory, Figures and tables supporting the main report, hut not immediately required, can be included in one or more appendices. Literature sources should be suitably referenced in the text, and references should he specified in a standardised manner, generally including author(s), book title and publisher or title (and volume) of journal and paper, year of publication, and relevant page numbers. All figures, tables and literature rel’erences (and appendices) should he explicitly referred to in the thesis. The evaluation of the master thesis will emphasise its clarity and thoroughness. It is also important that the author gives an independent presentation of the topic using views and insights developed in the thesis work.
Three weeks after the start of the thesis work, an A3 sheet illustrating the work is to be handed in. A template for this presentation is available on the 1PM website under the menu “Masteroppgave” (http://www. ntnu no/iprn/mastei’oppgave). This sheet shoti Id he updated one week before submission of’ the thesis. .
The thesis shall be submitted electronically via I)AIM, NTNIJ’s system for digital archiving and submission of rnastei’ theses.
Contact persons: At the department From the industiy
: Rjørn I1augen, Professor/Co—supervisor : LINKftr (contact person to be named by August 201 3)
j 7,ZEZ7 lorgeir Web flepd of Division /
•
NTNU Norges naturvitenskapelige universitet Institutt for produktutvikling og materialer
Gunnar I liirkegärd Proi’essor/Supervisor
L
S.
Preface
This Master’s thesis, titled Fatigue Assessment of Components Subjected to NonProportional Stress Histories, was written as my final work in Mechanical Engineering at the Norwegian University of Science and Technology (NTNU). It serves as a direct continuation of an indepth project work, completed in spring 2013. As a scientific thesis, this is the product of one intense year spent in the complex world of multiaxial fatigue. As my last assignment as a student at NTNU, it entails every bit of experience and knowledge I have gained throughout my years as a student.
c
V
There are several I would like to direct my utmost gratitude to. Special thanks go to my supervisor and professor Gunnar Härkegård. During interesting discussions, and through his powers of persuasion and commitment, I have now ventured deeper into the world of fatigue than I previously thought possible. I also wish to thank my family and girlfriend for all encouragement, patience and support.
Øyvind A. Bruun Trondheim, December 17th, 2013
I
Abstract The fatigue assessment of components subjected to complex loading histories is a challenging topic. Several criteria intended for use under multiaxial stressstates and nonproportional loading have been proposed by many researchers throughout the years. This thesis is intended as a critical review of the fatigue assessment of both proportional and nonproportional stress histories. A database consisting of 268 experimental tests for biaxial fatigue limits were collected from various sources. The compiled database spans 20 materials, ranging from carbon steels to cast irons. The data were evaluated using five multiaxial fatigue criteria and two separate assessment methods. The first assessment method is here described as the proportionalmethod, which is the assessment of relevant stressvalues based on extreme values occurring throughout a cycle. The second method, here simply called the ASMEmethod, is heavily inspired by the ASMEcriterion as stated by the ASME Boiler and Pressure Vessel code. The latter method determines the relevant stress values based on relative diﬀerences in stress components over time. In addition to the fatigue test data, a stress cycle provided from the industry is examined and discussed. The lack of readily available fatigue test data for validating purposes is a serious concern that is discussed here. The database provided in the appendix is intended to partially remedy this, and serve as a starting point for future research. A comparison of predictions, both criteria and methodologywise is also provided. The results and findings are then critically discussed. The research shows that the predictability of a fatigue criterion depends on both material and stressstate. For brittle materials such as the cast irons included in the assessment, the normal stress criterion provides excellent results. For carbon and low alloy steels, as well as the aluminium alloy 76ST61, shear stress criteria such as Findley yield more accurate predictions. The ASMEmethod increases the complexity of the fatigue assessment, but is shown to have a positive eﬀect on predictions for the Findley criterion.
II
Sammendrag Utmattingsanalyse av komponenter utsatt for komplekse spenningshistorier er et utfordrende tema. Flere kriterier beregnet for bruk ved fleraksede spenningstilstander og ikkeproporsjonal belastning er gjennom årene blitt foreslått. Denne masteroppgaven har til hensikt å gi et kritisk innblikk i utmattingsanalysen av spenningshistorier av både proporsjonal og ikkeproporsjonal natur. I den forbindelse ble det samlet en database bestående av totalt 268 eksperimentelt bestemte utmattingsgrenser for kombinerte belastninger. Utmattingsgrensene er fordelt på 20 ulike materialer og tilsammen 27 testserier. Disse ble så evaluert ved bruk av fem ulike utmattingskriterier og to forskjellige fremgangsmåter. Den ene fremgangsmåten er den klassiske, proporsjonale fremgangsmåten for å bestemme spenningsverdier som amplituder på. Denne metoden benytter seg av ekstremverdier som inntreﬀer gjennom hele spenningssyklusen sett over ett. Den andre metoden, baserer seg på ASMEkriteriet som gjengitt i ASME Boiler and Pressure Vessel Code. Sistnevnte metode beregner spenningsverdier basert på deres relative forskjeller over tid. I tillegg til utmattingsgrensene gjengitt i databasen, ble også en spenningssykel hentet fra industrien gjennomgått og diskutert. Manglende tilgang på testdata er en kilde til bekymring, og blir grundig diskutert. I den anledning er utmattingsdataene samlet i databasen gjengitt som vedlegg, og slik er de enkelt tilgjengelig for videre bruk. Resultatet av undersøkelsen indikerer at nøyaktigheten på prediksjonene fra et utmattingskriterium avhenger av både materiale og spenningstilstand. For sprøe materialer slik som støpejern, gir normalspenningskriteriet uovertrufne resultater. For karbonstål og lavlegerte stål samt aluminiumslegeringen 76ST61 gir skjærspenningskriterier som Findley de beste resultatene. For noen kriterier, da spesielt Findleykriteriet, bidrar ASMEmetoden til mer nøyaktige prediksjoner. I bruk bidrar ASMEmetoden til at utmattingsanalysen generelt blir mer utfordrende.
III
Nomenclature tˆ
critical point in time
I1
first stress invariant
X
arithmetic mean value of random discrete variable
a
support factor from FKMRichtlinie
b
support factor from FKMRichtlinie
fcrit
critical parameter (Findley)
fW,σ
constant used by FKM
fW,τ
constant used by FKM
k
Findley constant
M
mean stress sensitivity
mp
mean value of predictions
n
number of variables
Nf
cycles to failure
P
loading parameter
R
relationship between max. and min. stress
Rm
ultimate tensile strength
s
sample standard deviation
sp
sample standard deviation of predictions
T
length of stress history
[sec] [MPa]
[MPa]
[sec]
V
t
time
Xi
discrete variable
[sec]
Vectors and matrixes I1
first stress invariant matrix
n
unit normal vector
S
cartesian stress tensor
x
placement in a body
Greek Symbols α
phase shift
β
constant
φˆ
angle between xaxis and largest principal stress
λ
constant
ω
angular frequency
φ
azimuth angle between xaxis and unit normal vector
σ′
modified stress according to the ASME criterion
[MPa]
σh
hydrostatic stress
[MPa]
σf′
fatigue strength coeﬃcient
[MPa]
Σ
stress field for P=1
σ
normal stress
[MPa]
σ1,2
principal stresses
[MPa]
σA
purely pulsating fatigue limit for tension/bending
[MPa]
σW
fatigue limit for fully reversed normal stress
[MPa]
σar
equivalent fully reversed stress amplitude
[MPa]
σeq,T
Tresca equivalent stress
[MPa]
VI
[deg]
[◦ ]
[rad/sec] [◦ ]
σeq
von Mises equivalent stress
[MPa]
τ
shear stress
[MPa]
τA
fatigue limit for purely pulsating shear stress
[MPa]
τW
fully reversed fatigue limit in shear
[MPa]
θ
polar angle
S′
diﬀerence between principal stresses (ASME criterion)
[◦ ] [MPa]
Subscripts a
amplitude of given stress component
max
maximum value of a given stress component
min
maximum value of a given stress component
m
mean value of a given stress component
A, B
indication of case A or case B crack growth
ij
element of a given stress component in cartesian stress tensor
VII
Contents Preface
I
Abstract
II
Sammendrag
III
Nomenclature
IV
1. Introduction
1
1.1. Limitation of Investigation . . . . . . . . . . . . . . . . . . . . . . . .
2
1.2. Previous Research . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
3
2. Literature Review
5
2.1. Stress Analysis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
5
2.1.1. Static Stress Analysis . . . . . . . . . . . . . . . . . . . . . . .
5
2.1.2. Dynamic Stress Analysis . . . . . . . . . . . . . . . . . . . . .
7
2.1.3. Special Case of Plane Stress . . . . . . . . . . . . . . . . . . .
8
2.2. Uniaxial Fatigue Analysis . . . . . . . . . . . . . . . . . . . . . . . .
9
2.3. Multiaxial Fatigue Criteria . . . . . . . . . . . . . . . . . . . . . . . . 10 2.3.1. Normal Stress Criterion . . . . . . . . . . . . . . . . . . . . . 11 2.3.2. MisesSines Criterion . . . . . . . . . . . . . . . . . . . . . . . 11 2.3.3. TrescaSines Criterion . . . . . . . . . . . . . . . . . . . . . . 11 2.3.4. ASMECriterion for NonProportional Loading . . . . . . . . . 12 2.3.5. Findley Criterion . . . . . . . . . . . . . . . . . . . . . . . . . 13 2.3.6. Other Fatigue Criteria . . . . . . . . . . . . . . . . . . . . . . 14 2.3.6.1. Crossland Criterion . . . . . . . . . . . . . . . . . . . 14 2.3.6.2. McDiarmid Criterion . . . . . . . . . . . . . . . . . . 14 2.3.6.3. Matake Criterion . . . . . . . . . . . . . . . . . . . . 15 2.4. Statistical Analysis . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15 2.5. FKMRichtlinie . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15 3. Fatigue Test Database
17
IX
Contents 4. Procedure
21
4.1. General Procedure for Fatigue Assessment . . . . . . . . . . . . . . . 21 4.2. Normalizing of Stresses . . . . . . . . . . . . . . . . . . . . . . . . . . 22 4.3. Determination of Material Parameters and Constants . . . . . . . . . 22 4.4. Modelling of Stress Histories . . . . . . . . . . . . . . . . . . . . . . . 22 4.5. Proportional Method for Determination of Criteria . . . . . . . . . . 23 4.6. ASME Method for Determination of Criteria . . . . . . . . . . . . . . 23 4.7. Computational Algorithm . . . . . . . . . . . . . . . . . . . . . . . . 25 4.8. Failure Assessment Diagrams . . . . . . . . . . . . . . . . . . . . . . 27 4.8.1. Algorithm and Plotting . . . . . . . . . . . . . . . . . . . . . . 28 4.8.2. Material Parameters . . . . . . . . . . . . . . . . . . . . . . . 28 4.9. Fatigue Database . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 29 4.9.1. Selection Process . . . . . . . . . . . . . . . . . . . . . . . . . 29 4.9.2. Determination of Missing Parameters . . . . . . . . . . . . . . 29 4.10. StressCycle From Industry . . . . . . . . . . . . . . . . . . . . . . . 31 5. Results
33
5.1. Determination of Parameters . . . . . . . . . . . . . . . . . . . . . . . 33 5.2. Failure Assessment Diagrams . . . . . . . . . . . . . . . . . . . . . . 34 5.3. Predictions for Tests at the Fatigue Limit
. . . . . . . . . . . . . . . 35
5.3.1. Predictions for Selected Loading Cases . . . . . . . . . . . . . 35 5.3.2. Comparison of Predictions for Material Groups . . . . . . . . 40 5.4. StressCycle of Dynamically Loaded Component . . . . . . . . . . . . 43 6. Discussion
47
6.1. Requirements of a Fatigue Criterion . . . . . . . . . . . . . . . . . . . 47 6.2. Assessment and Suitability of Criteria . . . . . . . . . . . . . . . . . . 48 6.2.1. Normal Stress Criterion . . . . . . . . . . . . . . . . . . . . . 48 6.2.2. MisesSines Criterion . . . . . . . . . . . . . . . . . . . . . . . 49 6.2.3. TrescaSines Criterion . . . . . . . . . . . . . . . . . . . . . . 49 6.2.4. ASMECriterion . . . . . . . . . . . . . . . . . . . . . . . . . . 49 6.2.5. Findley Criterion . . . . . . . . . . . . . . . . . . . . . . . . . 50 6.3. Proportional Method vs ASMEMethod . . . . . . . . . . . . . . . . . 50 6.4. Fatigue Assessment of Stress Cycle . . . . . . . . . . . . . . . . . . . 52 6.5. A Note on the Availability of Fatigue TestData . . . . . . . . . . . . 53 6.6. Continued Work and Suggested Improvements . . . . . . . . . . . . . 54 7. Conclusion
X
57
Contents Bibliography
59
List of Figures
63
List of Tables
63
A. Material Data
67
B. Predictions
79
XI
1. Introduction "Structural engineering is the art of modelling materials we do not wholly understand into shapes we cannot precisely analyse so as to withstand forces we cannot properly assess in such a way that the public at large has no reason to suspect the extent of our ignorance."  Dr. A. R. Dykes [1] A correct prediction of the fatigue limit and lifetime of a component is of the utmost importance with respect to safety and cost issues. In order to address these challenges, models for fatigue assessment need to accurately predict fatiguelife. Many mechanical and structural components will throughout their life be subjected to loads of a timevarying nature, with stresses working in several directions. Typical examples are drive shafts in cars, turbine blades in jet engines and windmills. The resulting stress histories may be either proportional or nonproportional, and a number for multiaxial criteria intended for use under such conditions exist. However, the complexity of the fatigue assessment is considerably increased, and so these criteria may be impractical for the practicing engineer. As a result, these criteria are not yet widely implemented. Lately, with the advent of computational resources, the fatigue assessments are made considerably more manageable. Even at the time of writing this thesis, new criteria and algorithms are submitted to the scientific community for review. This thesis is meant to serve a number of purposes. Primarily, it concerns the fatigue assessment of experimental data collected from the literature. The tests are evaluated using selected criteria, and employed both using a proportional method and with an ASMEinspired method. The results are then presented, and the criteria are compared with respect to usability and accuracy of predictions. The topic of available experimental data is also addressed, and is an important aspect of this thesis. A thorough search for high cycle fatigue (HCF) tests was conducted, and the results were compiled in a database, spanning 20 diﬀerent materials and a total of 268 tests. This was necessary in order to provide a comprehensive comparison of the fatigue criteria. Although several such databases are known to
1
1. Introduction exist, very few are available for public use. As a result, new criteria are often evaluated for a statistically insignificant number of tests. Several other discrepancies and worrisome trends were encountered during the search, and is critically discussed later on. Occasionally the gathered tests were incomplete, in that they lacked relevant information regarding the uniaxial fatigue limit σA for purely pulsating loading. In these cases, FKMRichtlinie was used to approximate the mean stress sensitivity M from tablevalues and known fatigue limits. Since most of the criteria depend on these values, an aspect of this thesis became the quality of FKMderived values, and their impact on the fatigue assessment.
1.1. Limitation of Investigation During the investigation, very little fatiguecrack growth data was found. Focus was therefore shifted towards stressbased fatigue criteria and SN data. The performed analysis spans both shearstress criteria, and pure normal stress criteria. The shear stress criteria are here represented by the Sines, Findley and ASMEcriterion. Two versions of the Sines criterion are employed  one with the von Mises equivalentstress amplitude, and the other with the Tresca equivalentstress amplitude. The Findley criterion is here applied with the constant k determined by two possible methods. The ASMEcriterion as stated in the ASME Boiler and Pressure Vessel Code is included as well. In the normalstress category, one normal stress criterion based on the HempelMorrow line is implemented. All criteria, with the exception of the ASMEcriterion are implemented in two diﬀerent ways. Initially, they are implemented using the traditional, textbook method of assessment. Secondly, an assessment method based on the ASMEcriterion is proposed and evaluated. It was initially intended that nonproportional stress histories above the fatigue limit and suitable cyclecounting rules should be considered. Due to limitations in time, it was preferred to expand the database of tests regarding fatigue limits in the highcycle regime instead. The thesis therefore only concerns local stress based analysis, and mostly plane stresses (2Dstresses). A fatigue analysis of a dynamically loaded component is provided in order to provide a more comprehensive picture, as opposed to the planestress, constantamplitude stress states provided in the fatigue database.
2
1.2. Previous Research
1.2. Previous Research Many comparable analyses have been performed by a plethora of authors. Notable contributions in the field are the works of Papadopoulus [2] and Carpinteri [3]. Previous research in the area at NTNU were performed in 1980 by Nøkleby and published in his phdthesis [4]. Large databases of fatigue limits for proportional and nonproportional loading have been gathered by Papuga on his webpage [5], and by Troost et al. [6]. Experimental data collected from the latter paper have been used in this thesis. One might conclude that such analyses are neither new nor original, as they have been performed to a great eﬀect by several authors in the past. What sets this thesis apart from similar works is the amount of experimental data used for verification, and the addition of a proposed ASMEinspired assessment method. The data used in this thesis are also enclosed in the appendix. In that respect it might serve as a starting point for future investigations at NTNU.
3
2. Literature Review A summary of the literature reviewed is given here. The information provided in this chapter spans from stress analysis, to the fatigue criteria used in the stress analysis. A description of the fatigue database containing collected data is also included in this chapter, but is further explained later on, as several additions (newly calculated parameters) are described in chapter 4  Procedure.
2.1. Stress Analysis A comprehensive knowledge of mechanics and stressanalysis is recommended to fully understand the following theory. This section is not an extensive explanation of the subject. It is intended rather, to give a short and clear summary of basic theory needed to implement the fatigue criteria presented in section 2.3. For a more indepth explanation, the works of Dowling [7] and Marquis, Socie [8] are recommended.
2.1.1. Static Stress Analysis For the case of 3Dstresses, the stresses at a point x is given by the Cartesian stress tensor S given in (2.1), ⎡ ⎤ σx τxy τxz ⎢ ⎥ S = ⎣ τyx σy τyz ⎦ (2.1) τzx τzy σz where the equal indexes i = j define a normal stress, and unequal stresses i ̸= j define a shear stress. The normal stresses are here given with only one index, i.e x instead of xx due to practicality. The unit normal vector originating in the point x, and characterized by the polar angle θ with the yaxis and with the azimuth angle φ with the xaxis in a 3D
5
2. Literature Review z
θ
. φ
y
x
Figure 2.1.1.: 3Dcoordinate system.
coordinate system as shown in figure (2.1.1) can be written as nT =
'
sinθcosφ sinθsinφ cosφ
(
(2.2)
and the tension vector on a plane normal to the vector n is given by (2.3)
s = Sn
The normal and shear stress on the plane with unit normal vector n become σ = nT s = nT Sn
τ = s − σn
(2.4)
The magnitude of the shear stress vector τ given in (2.4) can be computed as given by (2.5). τ 2 = τ T τ = (s − σn)T (s − σn) = sT s − σ 2 (2.5) The principal stresses σ1 , σ2 and σ3 for a 3Dstate of stresses are found by solving equation (2.6) with respect to σ. 2 2 2 σ 3 − σ 2 (σx + σy + σz ) + σ(σx σy + σy σz + σx σz − τxy − τyz − τxz )
2 2 2 − (σx σy σz + 2τxy τyz τzx − σx τyz − σy τzx − σz τxy ) (2.6)
6
2.1. Stress Analysis
2.1.2. Dynamic Stress Analysis For stresses varying over time, the stress state can be expressed by introducing the parameter P(t) describing the load history over time. Each of the stress components in S from (2.1) now take the form of equation (2.7). σij (x, t) = P (t)Σij (x)
(2.7)
where x designates at which point the stresses are working, t is the point in time and Σij (x) is the stress field in point x for P = 1. A basic alternating and cyclic stress state based on a sinusoidal wave is possibly the easiest case of time varying stresses. The parameter P(t) can be expressed as a sinusodial wave function when written as P (t) = Pm + Pa sin(ωt). For proportional loading, the stress components given in S all vary with the same ratio. This corresponds to the same P(t) valid for all components of S, so that each of the components may be expressed by equation (2.8), σij (x, t) = σij,m (x) + σij,a (x)sin(ωt) (2.8) where σij,m is the mean stress, σij,a is the stress amplitude and ω is the angular frequency. Since the same ω applies for all stress components, the loading is proportional. As a result, the principal stresses maintain a fixed position with the x, y and z axis. The concept of nonproportional loading can be explained by introducing angular frequencies ωij and phaseshifts αij for each individual component in S. The parameter describing the load history now takes the form of Pij (t) = Pm + Pa sin(ωij t − αij ), with the stress components given as σij (x, t) = σij,m (x) + σij,a (x)sin(ωij t − αij )
(2.9)
The ratio between the stresscomponents may now vary with time, and the principal stresses can change orientation. Other variations of nonproportional loading might occur when Pij (t) is a completely random value. For constantamplitude loading described in equation (2.8) and (2.9), the cyclic amplitude stress and the constant mean stress can be found from (2.10) and (2.11), 1 σa = [σmax − σmin ] 2 1 σm = [σmax + σmin ] 2
(2.10) (2.11)
7
2. Literature Review
where σmax and σmin are the maximum and minimum values of the stress component occurring throughout a cycle. The stress ratio R between the maximum and minimum values is given as σmin R= (2.12) σmax and thus for fully reversed stresses with σmin = −σa and σmax = σa the Rratio is equal to −1. For purely pulsating stresses with σmin = 0, the ratio R = 0.
2.1.3. Special Case of Plane Stress The case of plane stress is specifically described here as all cases calculated further on are valid for σz = 0 and θ = π2 . The principal stresses previously now take on the less challenging form given in (2.13).
σy τxy
τ (φ)
y σx
x
.
σx
σ(φ) φ
σx
x
y τxy
τxy σy
σy
Figure 2.1.2.: Element showing stress components for plane stress, σz = 0.
σ1,2
σ x + σy = ± 2 1
)
(
σx − σy 2 2 ) + τxy 2
(2.13)
With the angle φˆ between the largest principal stress σ1 and the xaxis given in (2.14). 1 2τxy φˆ = arctan( ) (2.14) 2 σx − σy The normal stresses (2.15) and (2.16) modified for plane stress are given as
8
σ(φ) = σx cos2 φ + σy sin2 φ + 2τxy sin φ cos φ
(2.15)
τ (φ) = (σy − σx ) sin φ cos φ + τxy (cos2 φ − sin2 φ)
(2.16)
2.2. Uniaxial Fatigue Analysis
2.2. Uniaxial Fatigue Analysis Fatigue assessment is the analysis of damage caused by varying stresses over time. The allowable cyclic stresses in order to avoid fatigue failure are determined by the fatigue limit, which are dependent on the material. In the literature it is diﬀerentiated between shear stress criteria, and normal stress criteria  each type utilizing a diﬀerent fatigue limit. For plane stress, a failure locus depicting the boundaries of failure can be drawn, see figure (2.2.1).
σ2
(σW , σW )
.
σ1
τmax
(σW , σW )
Figure 2.2.1.: Failure locus showing the fatigue limits for fully reversed stresses in shear and normal stress. The grey area in figure (2.2.1) show the boundaries between a pure shear stress case, and a pure normal stress case. According to the principal stress criteria, a fully reversed normal stress amplitude must be beneath the fatigue limit of the material for fully reversed stresses, σW . The shear stress criterion states that the fatigue limit in shear for R = −1 is equal to one half of the fatigue limit for normal stress, τW = 12 σW . The uniaxial fatigue limit for a uniaxial stress cycle with amplitude and mean stresses can be written as the HempelMorrow line given in (2.17), σa σm + ′ =1 σW σ f
(2.17)
where σ ′ f is a constant. Equation (2.17) is1 plotted in the Haighdiagram provided in figure (2.2.2), along with lines for several stressratios. The mean stress sensitivity M, which expresses how sensitive the fatigue limit for purely pulsating stresses, σA is to mean stresses is given by equation (2.18) and
9
2. Literature Review σa R=0
R = −1
σW σA
M =0
σ a + σ m = Rm M = 0.25
.
M =1 Rm
σm
Figure 2.2.2.: Haighdiagram. plotted in the Haighdiagram as well. M=
σW −1 σA
(2.18)
Equation (2.18) is valid for fatigue limits in both shear and normal stresses. It is however in this thesis only used in combination1 with the fatigue limits of normal stress.
2.3. Multiaxial Fatigue Criteria The fatigue models presented here are all on the form given in equation (2.19), and follows the equivalent stress approach where an equivalent stress amplitude σar is calculated from multiaxial stresses. σar = f (σij , . . .) ≤ σW
(2.19)
It follows that σar is the equivalent uniaxial, fully reversed stress amplitude determined by the function f, which depends on the criteria and the combination of stresses f (σij , . . .). The determination of σar is dependent on the individual criterion. When σar is found, it can be compared with σW , and failure is predicted when σar surpasses σW . The criteria utilized in this thesis are either normalstress criteria or shear stress criteria. They can further be divided into criticalplane criteria, stressinvariant criteria, and principalstress based criteria.
10
2.3. Multiaxial Fatigue Criteria
2.3.1. Normal Stress Criterion The simplest criterion presented here is the normal stress criterion [9]. By combining the HempelMorrow line given in (2.17) with the mean stress sensitivity M (2.18), the criterion can shown to be expressed as σar = max[σa (φ) + M σm (φ)] ≤ σW
(2.20)
As is apparent from (2.20), only normal stresses on an arbitrary plane are examined. For constant amplitude stresses, both the amplitude and mean stress component throughout the whole cycle are used. Fatigue failure is expected to occur on the plane exposed to the largest combination of stresses. Thus, the plane which maximises the expression σa (φ) + M σm (φ) is defined as the criticalplane, and the corresponding angle between the x axis and normal vector n orthogonal to the plane is designated φcrit (for plane stresses).
2.3.2. MisesSines Criterion Sines proposed a criterion intended for inphase multiaxial proportional stresses in the 1950s [10]. The criterion as it is used here is given in (2.21), σar = max[σeq,a + M I1 ] ≤ σW
(2.21)
with σeq beeing the von Mises equivalent stress amplitude expressed as σeq,a =
*
2 + σ 2 − σ σ + 3τ 2 σxa xa ya ya xya
(2.22)
and the first stress invariant I1 given by I1 = σxm + σym
(2.23)
Both I1 and σeq are here expressed only for plane stress. Both being stress invariants, their validity for nonproportional outofphase stresses must be taken into account.
2.3.3. TrescaSines Criterion A modification of the existing Sines criterion is proposed by Härkegård [9] by using the Tresca equivalent stress amplitude σeq,T,a = 2τa,max instead of the von Mises
11
2. Literature Review stress amplitude. σar = max[2τa (φ)] + M I1 ≤ σW
(2.24)
In contrast to the MisesSines criterion, the shearstress on an arbitrary plane are examined. Following the previous procedures, the plane which maximises a combination of stresses are found. Since the stress invariant I1 is equal in all directions, the critical plane coincides with the maximum shear plane throughout a cycle.
2.3.4. ASMECriterion for NonProportional Loading Two criteria for multiaxial fatigue stressbased analysis are proposed by the ASME (American Society of Mechanical Engineers) Boiler and Pressure Vessel Code. Only the ASMEcriterion for nonproportional loading is presented here, the other one being valid for proportional loading only and the two being identical for such cases. The criterion as it is stated here is taken from [11] and [8]. The ASMEcriterion for nonproportional loading may be expressed as follows: 1. Calculate the values for each of the six stress components given in the stress tensor S, (2.1) over time. 2. Determination of a point in time tˆ = [ 0, T ], where the conditions are extreme and T is the length of the stresshistory. If this point in time is not known a priori, several points in time need to be examined in order to find the one that yields the largest alternating stressamplitude σar . 3. Determine the stress diﬀerence between the stress components in S occurring at tˆ and every other possible point in time t = [ 0, T ]. This is done by subtracting the stressvalue occurring at tˆ from the stress values occurring at t. The resulting stress component is called σij′ . σij′ = σij (t) − σij (tˆ)
(2.25)
4. Calculate the modified principal stresses σ1′ , σ2′ derived from the six components σij′ for each point of time during the cycle. Equation (2.13) is used for plane stresses. ′ ′ ′ 5. Determine the stress diﬀerences S12 = σ1′ − σ2′ , S23 = σ2′ − σ3′ , S31 = σ3′ − σ1′ versus time, and find the largest absolute magnitude of any stress diﬀerence of any point in time. The alternating stress amplitude according to ASME, is
12
2.3. Multiaxial Fatigue Criteria then one half of this magnitude. 1 ′ ′ ′ σar = max( S12 ,  S23 ,  S31 ) ≤ σW 2
(2.26)
Nowhere is it specifically stated how to implement the criterion for stress states where nonzero mean stresses are present. Suitable modifications of mean stress are not covered here.
2.3.5. Findley Criterion The Findley criterion originated in the late 50’s is a criticalplane criterion where a linear combination of stresses acting on an arbitrary plane is considered [12]. The general background follows the assumption that shear stresses acting on a plane are the key cause of crack initiation and failure. The maximum normal stress acting on the same plane only amplifies the damaging eﬀect from the shear stresses, and is thus taken into account as well. The criterion as it was originally presented is given in equation (2.27). The damage parameter f is a function of both shear and normal stress occurring on an arbitrary plane, and thus the critical plane is the plane which maximises the combinations of stresses given in (2.27). f = max[τa (φ) + kσmax (φ)] ≤ fcrit
(2.27)
The constant k and the critical multiaxial fatigue parameter fcrit need to be determined by solving (2.27) for at least two uniaxial cases, where only one stress component is present. Input of the corresponding uniaxial fatigue limits for both fully reversed (R = −1) and purely pulsating (R = 0) yield the four equations (2.28). ⎧σ √ W ⎪ [ k 2 + 1 + k] ⎪ ⎪ 2 ⎪ ⎪ ⎪ ⎨ σA √ 2 [ 4k + 1 + 2k] f= 2 √ ⎪ ⎪ ⎪ τW [ k 2 + 1] ⎪ ⎪ ⎪ ⎩ √ 2 τA [ 4k + 1
R=1
(2.28a)
R=0
(2.28b)
R=1
(2.28c)
R=0
(2.28d)
The parameters k and fcrit are then found by setting two of the expressions given in (2.28) equal to each other, i.e f (σW ) = f (σA ) corresponding to equation (2.28b)=(2.28c) and solving for k and fcrit .
13
2. Literature Review The original criterion can be rewritten as (2.29) using (2.28b), where the f and fcrit are replaced by σar and σW . For the sake of comparison, this is the version used in later calculations. τa (φ) + kσmax (φ) √ σar = max( 1 ) ≤ σW (2.29) (k + 1 + k 2 ) 2 The Findley criterion leaves the user a choice in which fatigue limits one can use to determine the constants k and fcrit . Previous examinations (REF) have shown that the combination of these four equations in (2.28) does not yield a unique solution, and since the user may determine the constants based on any two known fatigue limits, k and fcrit vary accordingly.
2.3.6. Other Fatigue Criteria The five previous criteria are only a selection of the wide array of available options. The following sections present additional models for assessing proportional and nonproportional loading, but were not used in the later fatigue assessment. 2.3.6.1. Crossland Criterion The Crossland criterion [13] is a stressinvariant criterion similar to the MisesSines criterion. It uses the von Mises stress amplitude given in (2.22) in combination with the maximum hydrostatic stress σh,max . σeq,a + λσh,max ≤ β
(2.30)
The constants λ, β are determined by solving the expression (2.22) for simple uniaxial cases and input of the corresponding fatigue limits. 2.3.6.2. McDiarmid Criterion The McDiarmid criterion [14],[15] utilizes the maximum shear and normal stress occurring on a plane throughout a cycle. The critical plane is defined as the plane where the largest shear stress amplitude occurs, and not the plane which maximises a combination of stresses (as opposed to the Findley and Normal Stress criterion). The criterion is given in (2.31). max(
14
τa (φ) σa (φ) )+ ≤1 τA,B Rm
(2.31)
2.4. Statistical Analysis The criterion stands out from the other presented criteria as the shear fatigue strength for either Case A or Case B cracking is used to scale the maximum shear stress. Cracks for Case A propagate parallel along the surface of a component, and Case B cracks propagate into the component from the surface. For combined loading, cracks are developing according to Case A, and τA,B is equal to the fatigue limit in shear for fully reversed stresses, τA,B = τW . 2.3.6.3. Matake Criterion The criterion proposed by Matake [16] is very similar to the Findley criterion, but diﬀers in the definition of critical plane, which is stated to be the maximum shear plane. max{τa (φ)} + λσmax (φ) ≤ β (2.32) As in the Crossland criterion, the constants λ, β are determined by solving the expression given in (2.32) for uniaxial cases and input of the corresponding fatigue limits. This results in a criterion which is less computationally expensive, as the constants are easier to determine in addition to that the critical plane may be found relatively easy for simple stress states.
2.4. Statistical Analysis Some statistical parameters are used to better present the results. They are presented as given in [17] and provided here for further reference. The arithmetic mean value X of n discrete, random variables are given in (2.33), where Xi is one of n discrete variables. n 1/ X= Xi (2.33) n i=n The sample standard deviation s is a measure of the degree of spread, and is expressed in (2.34). 0 1 n 1 1 / s=2 (Xi − X)2 (2.34) n − 1 i=n
2.5. FKMRichtlinie FKMRichtlinie [18, 19] provides solutions and useful experimental approximations of parameters relevant to fatigue assessment. It is mainly used here to determine the
15
2. Literature Review mean stress sensitivity M when no σA is available. M is given by equation (2.35), with support factors depending on the material provided in table 2.1. It is worth noting that the M is valid for 106 cycles. (2.35)
M = a · 10−3 Rm + b
The fatigue limits in shear and normal stresses for fully reversed loading may be approximated by equation (2.36) and (2.37) using tabular values given in table 2.1. (2.36)
σW = Rm · fW,σ
(2.37)
τW = σW · fW,τ
Table 2.1.: Support factors for types of material groups according to FKMRichtlinie. Material group Eng. Translation fW,σ fW,τ a b Einsatzstahl Unalloyed/low alloy steels Stahl ausser diesen Other steels GS Nodular graphite cast iron GJL Lamellar graphite cast iron Aluminiumknetwerkstoﬀ Wrought aluminium
0.40 0.45 0.34 0.34 0.30
0.577 0.35 0.1 0.577 0.35 0.1 0.577 0.35 0.05 1.0 0.0 0.5 0.75 1.0 0.04
The mean stress sensitivity given in (2.35) may be used in combination with the HempelMorrow line in equation (2.17) to determine the uniaxial fatigue limit for pure pulsating stress σA .
16
3. Fatigue Test Database Due to their importance, the fatigue tests assessed in this thesis are presented in a chapter of their own. It contains 268 fatigue limits determined for both combined and uniaxial loading cases. An overview of the materials is given in tables (3.1) and (3.2), together with calculated material parameters relevant to the fatigue assessment. All fatigue tests are valid for the HCFregime, with cycles ranging from 106 and upwards. The tests were all performed on unnotched, solid or hollow specimens, as specified in table (A.1). The materials are roughly divided into three categories carbon and low alloy steels, aluminium alloys, and cast irons. The selection process is further explained in section 4.9. As the fatigue test data collected and assessed in this thesis grew, it became apparent that some assumptions needed to be made. All materials were therefore assumed to be isotropic materials, with no cyclic eﬀects such as isotropic or kinematic hardening. Perhaps the most influential assumption was the indiﬀerence to loading, as opposed to the resulting stresses. As rotated bending, plane bending, and tension both yield a normalstress, these were treated as equal. The fatigue limits were however chosen to correspond to the loading case when available. No discrimination was done with respect to the determination of corresponding material parameters from FKMRichtlinie.
17
3. Fatigue Test Database
Material
A.2 A.4 A.5 A.6 A.8 A.5 A.8 A.11 A.7 A.7 A.7 A.4 A.11 A.4 A.6 A.2 A.6 A.8 A.3 A.9
424.6 262.5 149.0 0.57 520.0 310.0 179.0 0.58 518.8 235.4 137.3 0.58 395 206 123 168.5 0.60 765.2 295 182 264 0.62 704.1 313.9 196.2 0.63 706 313 213 245 0.68 520 332 186 0.56 710 343 204 265 0.59 795 410 256 320 0.62 858 415 259 320 0.62 1160 660 410 0.62 1200 690 428 0.62 780 361 228 300 0.63 780 361 228 300 0.63 1000.8 583.8 370.7 0.63 1025 398 260 310 0.65 801 340 228 300 0.67 895.5 540.5 352.1 0.65 902 382 283.5 311 0.74
0.049 0.082 0.082 0.223 0.117 0.146 0.278 0.082 0.294 0.281 0.297 0.306 0.320 0.203 0.203 0.250 0.284 0.133 0.213 0.228
250.3 286.5 217.6 (198.4) (252.6) 273.8 (272.9) 306.8 (298.7) (348.0) (345.7) 505.4 522.7 (307.8) (307.8) 466.9 (316.2) (288.1) 445.4 (314.2)
0.048 0.079 0.079 0.211 0.113 0.140 0.264 0.080 0.280 0.267 0.283 0.292 0.306 0.193 0.193 0.238 0.270 0.128 0.202 0.216
0.136 0.157 0.169 0.198 0.241 0.258 0.387 0.121 0.193 0.257 0.256 0.250 0.248 0.273 0.273 0.280 0.322 0.363 0.318 0.554
Table 3.1.: Given and calculated material parameters for carbon steels and alloyed steels. Tests Material parameters from literature Calculated material parameters σW given in Rm σW τW σA σA M k(σA ) k(τW ) table MPa MPa MPa MPa τW MPa Ref.
Carbon and low alloy steels 0.1 % C Steel [20] XC18 Steel [21] Mild Steel [3] St35 Steel [22] St60 Steel [6] Swedish Hard Steel [3] Ck 35 V [6] C20 annealed Steel [23] 34Cr4 (1) [22] 34Cr4 (2) [22] 34Cr4 (3) [22] 30CrMo16 (1) [24, 21] 30CrMo16 (2) [23] 25CrMo4 (1) [21] 25CrMo4 (2) [22] S65A [25] 42CrMo4 [22] 25CrMo4 (3) [6] 3.5% NiCr steel [20] 34CrMo4 V [6]
() Stress values are calculated for comparability but not used in later calculations.
18
19
230.1 795 294 230
Nodular graphite cast irons “Silal” cast iron [20] A.3 ENGJS8002 [23] A.11
Lamellar graphite cast irons GG30 [6] A.9 Cast iron [3] A.5 148 96.1
230.1 294
217.9 188.2 170.3
135 91.2
199.2 220
143.4 119.3 109.6 0.87 0.75
0.66 0.63 0.64
102.5 0.91 0.95


0.444 0.500
0.161 0.358
0.460 0.438 0.396
(98.7) 64.1
198.2 216.5
149.2 130.9 122.0
() Stress values are calculated for comparability but not used in later calculations.
499.9 499.9 499.9
A.10 A.10 A.10
Aluminium alloys 76ST61 (1) [26] 76ST61 (2) [26] 76ST61 (3) [26]
0.441 0.509
0.153 0.345
0.460 0.433 0.386
1.456 2.041
1.073 0.572
0.332 0.278 0.300
Table 3.2.: Given and calculated material parameters for aluminium alloys and cast irons. Tests Material parameters from literature Calculated material parameters σW Material Ref. given in Rm σW τW σA σA M k(σA ) k(τW ) table MPa MPa MPa MPa τW MPa
4. Procedure 4.1. General Procedure for Fatigue Assessment The procedure for the fatigue assessment of proportional and nonproportional stresses may diﬀer depending on the criterion. In order to evaluate all criteria simultaneously, a general algorithm was needed. An overview of the algorithm such as it was implemented is given below. Some steps are elaborated further in the following sections. The algorithm is described for the special case of plane stress, but may be expanded to involve threedimensional stresses with minimal eﬀort. 1. Determination of any material parameters relevant for the fatigue assessment. This involved constants, fatigue limits and mean stress sensitivityvalues. 2. Determination of the three stress components σx , σy and τxy , over time. In this case, the stress history was either provided beforehand, or was modelled as a constantamplitude sinusoidal function. 3. Computation of the principal stresses σ1 and σ2 given in (2.13) over time. 4. Calculation of the stresses σ(φ), τ (φ) given in (2.15) and (2.16) on every plane φ ∈ [ 0, 180◦ ] with a step of 1◦ over the course of the whole stress history. 5. Calculation of stress amplitudes σxa , σya , τxya , σa (φ), τa (φ), and the mean stresses σxm , σym , τxym , σm (φ), τm (φ). 6. Computation of stress terms such as the stress invariant I1 from (2.23) and the von Mises equivalent stress amplitude (2.22). 7. Evaluation of the fatigue criteria from all relevant values determined in the previous steps. This general algorithm describes the steps followed in order to evaluate all criteria utilized here. It follows that some steps are redundant for some, as the computation of I1 is essential for MisesSines and TrescaSines, but not necessary for the Findley criterion.
21
4. Procedure
4.2. Normalizing of Stresses The fatigue criteria presented in section 2.3 can all be normalized with respect to σW . All criteria can now be rewritten according to equation (4.1). σar ≤1 σW
(4.1)
The predictions provided by the criteria are now dimensionless, where failure is ar predicted when σσW > 1. Further it can be shown that the coordinate stresses used as input now take the form of normalized values σσWx , σσWy and στxy . Advantages when W normalizing stresses in this way is the ability to directly compare predictions between diﬀerent materials and criteria. An added bonus is the more intuitive presentation of the magnitude of a stressvalue relative to the fatigue limit.
4.3. Determination of Material Parameters and Constants FKMRichtlinie was used to determine the mean stress sensitivity M for cases where it was previously unknown. M was calculated by using appropriate constants for the materials, given in table 2.1 and equation (2.35). The fatigue limit for purely pulsating loading σA could then be computed using M in combination with (2.18). The Findley constant k was determined by using the fully reversed fatigue limit σW in combination with either σA or τW . They were calculated using the corresponding equations given in (2.28), so for k determined with the two normal stress fatigue limits, equations (2.28b) and (2.28c) were used. The determined parameters are given as either k(σA ) or k(τW ), where σA and τW denotes which fatigue limits in addition to σW were used.
4.4. Modelling of Stress Histories The fatigue test data compiled in chapter 3 were all reported to originate from investigations where the loading was modelled as a sinusoidal wave with constantamplitude stresses. The stresses in the calculations are therefore modelled using equation (2.9), here reproduced for ease of access. σij (x, t) = σij,m (x) + σij,a (x)sin(ωij t − αij ) 22
4.5. Proportional Method for Determination of Criteria The nonproportionality of the fatigue tests are caused by various phase shifts α 3 4 [◦ ]. The angular frequency ω rad were all reported to be equal for the stress sec components σij , and was set to a value of one. The length of the stress history was chosen to include at least 3 cycles. Since the period of a sine wave is given as in equation (4.2), 2π period = (4.2) ω this corresponds to a length T = 6π sec ≈ 18.8 sec. A length was chosen as T = 20 sec, and deemed suﬃcient both with respect to predictions ' and computing( time. The step was set to 1 seconds, forming a timevector as t = 0 1 · · · 20 seconds. The choice of T for constant amplitude stresses has no eﬀect on predictions as long as one full cycle is included in the stress history. It does however have an eﬀect on computing time, as it is desired to compute stresses for as few points in time as possible.
4.5. Proportional Method for Determination of Criteria Most of the criteria presented here are deduced for proportional, constant amplitude loading. The determination of the mean and alternating stress components is based on maximum and minimum values of the stresses, occurring throughout the whole cycle, as given in equation (2.11) and (2.10). For nonproportional loading, the maximum and minimum values used to determine the amplitudes and mean stresses may occur at severely diﬀerent points in time, and thus the variations in stresses (local maxima and minima) may not be taken suﬃciently into accord. This method is hereby referred to as the proportional method, as opposed to the proposed ASMEmethod for determination of stress parameters presented in sthe following section.
4.6. ASME Method for Determination of Criteria The proportionalmethod of assessing the criteria deals with constantamplitude loading. An alternative method inspired by the ASMEcriterion for assessing multiaxial fatigue criteria is proposed, where the parameters used for fatigue calculation are determined for a restricted interval in time. The stressparameters defined on each interval are hypothesised to have a specific relevance to each other, and thus yielding more accurate predictions.
23
4. Procedure 1. Compute the six stress components σx , σy etc. given by the Cartesian stress tensor S for the whole cycle or stress history. The length of the stress history measured in seconds can be denoted T. 2. Divide the resulting stress histories into steps, i.e steps of 1 second each when dealing with a stress history measured in seconds. When dealing with sinusoidalfunctions, steps of radians may also be used. 3. The ASMEcriterion states that a point in time where the conditions are extreme should be chosen, or when these are not easily identifiable that several points in time should be tried. When using the ASMEinspired assessment method however, combinations of parameters contained in each individual criar terion influence the σσW . As a result it might be challenging to pinpoint which points in time corresponds to the maximum prediction value. It is highly recommended that every possible combination is tried and tested. The point in time where the conditions are extreme can be denoted tˆ, and can be described by the vector tˆ ∈ [0, T ]. 4. The stress parameters used by the criteria are then calculated for each potential critical point tˆ relative to each point in time t ∈ [tˆ, T ]. The stress parameters are computed based on the stresses at the end points of the interval [ tˆ, t ]. Stress amplitudes and mean stresses are calculated according to (4.3) and (4.4). Notice that the absolute value of the stress diﬀerence is used when amplitudes are evaluated. 1 σa (tˆ, t) =  [σ(tˆ) − σ(t)] 2 1 σm (tˆ, t) = [σ(tˆ) + σ(t)] 2
(4.3) (4.4)
Maximum and minimum stresses on the interval [ tˆ, t ] are found as σmax = max[σ(tˆ), σ(t)]
(4.5)
σmin = min[σ(tˆ), σ(t)]
(4.6)
5. The calculated stress components may be placed in matrixes where tˆ is the number of rows and t is the number of columns. Such a matrix is here exampled
24
4.7. Computational Algorithm for stressamplitudes. ⎡
⎢ ⎢ ⎢ σ ija (tˆ, t) = ⎢ ⎢ ⎣
σij,a (0, 0) σij,a (0, 1) · · · σij,a (0, T) .. . σij,a (1, 1) .. . σij,a (T, 0) σij,a (0, T)
⎤ ⎥ ⎥ ⎥ ⎥ ⎥ ⎦
(4.7)
6. Other parameters such as the stress invariant I1 are also calculated intervalwise, so that I1 (tˆ, t) = σxm (tˆ, t) + σym (tˆ, t) for plane stress. The same goes for the von Mises stress amplitude σeq,a . 7. When dealing with criticalplane criteria where the critical plane is unknown, the relevant stress parameters occurring on φ ∈ [0, 180◦ ], i.e σmax (φ), τa (φ) (for plane stress) need to be determined intervalwise as described in step 4. 8. The fatigue criteria may now be evaluated for every interval when all relevant meanvalues, amplitudes, maximum and minimum values are calculated for every combination of tˆ ∈ [0, T ] and t ∈ [tˆ, T ]. An example is provided using the MisesSines criterion. σar = max[σ eq (ˆt, t) + M I1 (tˆ, t))] ≤ σW (ˆt,t)
(4.8)
The combination of [ tˆ, t ] yielding the largest σar , denoted σar,max is then assumed to give the largest contribution to fatigue damage. This method can be utilized for a wide range of criteria, both those based on stressinvariants and criticalplanes. It does however require a large amount of calculations to be done. It is especially challenging for the criteria where the criterion needs to be evaluated for every interval, on every possible plane.
4.7. Computational Algorithm The calculations done in this thesis were many and often extensive. The sheer amount of calculations meant that this task would be better executed by software. The several types of software were chosen out of availability, and previous experience. Microsoft Excel 2011 was used to store, and to a degree sort the collected data. Solving of intricate equations were done in the technical computing software Maple, version 16. For the major calculations, MATLAB R2013a was used. MATLAB
25
4. Procedure has the ability to read and write values from Excel, and this close integration was necessary in order to eﬀectively evaluate the test data. It was decided that a modular approach, with several interlinking scripts and each one performing a distinctive task, provided the best overview. A modular build was decided upon, where several individual scripts were linked together. This ensured a transparent process, where each script had only one specific task to fulfil. The scripts utilized can be grouped into two categories, mainscripts and supportingscripts. The main scripts were responsible for compiling the essential functions needed in order to perform the fatigue assessment as a whole. The supportscripts each had a specific function to fulfil, and were called by the mainscripts when needed.
Material Database This was a large excel document where fatigue tests collected from the literature were assembled. Information about stresses, stressratios, material constants etc. were precalculated and inserted into the database.
Support 1  SORT The SORT script, loaded values and information from the material database into MATLAB. It then and sorts all the fatigue tests according to a preset preference, i.e all tests where Rx = −1 and αxy = 0◦ . The preferences could be changed according to specific needs.
Support 2  CALC I This script uses input values provided from one of the four main scripts to construct a stress history. The stress history is then evaluated using the fatigue criteria and their original method of assessment. It is designed so that it may run in a loop, which is required from both the FAD and the FATDATAscript. The calculated values are then exported back to a main script.
Support 3  CALC II This script worked the same way as CALC I, but the tests were evaluated using the ASMEmethod to assess the stress history.
Main script 1  BASIC This is the simplest script utilized. It is mainly used to check single fatigue tests with control calculations, and also to determine specific stress combinations. It requires input of material parameters, and links to the calculationscript (CALC). The resuls may then plotted.
26
4.8. Failure Assessment Diagrams Main script 2  FAD The script uses either of the support scripts CALC I and II in a loop for various combinations of normalized coordinate stresses. The results are plotted as the diagrams shown in section 5.2. Main script 3  FATDATA The FATDATAscript retrieves values from the SORTscript, then evaluates each of them using CALC I or II run in a loop. The mean value and standard deviation of predictions from the criteria are then calculated. Main script 4  STRESSHIST The STRESSHISTscript loads a previously known stress history from Excel into MATLAB. It links to CALC I or II for assessment.
4.8. Failure Assessment Diagrams A visual presentation of a fatigue criterion provided on the normalized form given in ar (4.1) can be made by calculating the σσW values for combinations of the normalized σxa σxm τxya τxym stress components σW , σW , σW , σW , and plotting a line corresponding to a chosen σar value. At the fatigue limit σW , this value is equal to one and the plotted line σW corresponds to the limiting state of nonfailure predicted by the criterion. Diagrams of this type are hereby referred to as failure assessment diagrams (FAD). The area beneath the curve represents all combinations of coordinate stresses predicted to not cause fatigue failure. An example of such a diagram is given in figure 4.8.1. Failure Assessment Diagram 1
τxya / σW
0.8 Failure is predicted.
0.6
Criterion
0.4 No failure predicted.
0.2 0
0
0.2
0.4 0.6 σxa / σW
0.8
1
Figure 4.8.1.: Example of a failure assessment diagram for the TrescaSines criterion.
27
4. Procedure The biaxial fatigue limits collected in the material database can, when normalized, be plotted in a FAD along with a criterion. For a criterion that correctly predicts fatigue behaviour, the plotted fatigue limits are expected to lie on, or in the immediate vicinity of the plotted line. Fatigue limits from experimental data, which when plotted lie beneath the curve, show graphically that the prediction done by the criterion is nonconservative. Subsequently, a plotted fatigue limit above the curve corresponds to a conservative prediction.
4.8.1. Algorithm and Plotting As previously mentioned, the FAD’s were plotted by calculating the corresponding σar for a combinations of the normalized coordinate stresses. The values for the σW amplitude and mean stress components were chosen to range from 0 to 1.1 with a step of 0.1 as given in equation (4.9). Each combination of stresses was calculated by the FADscript described in section 4.7 using the general algorithm provided in section 4.1. σija σW
=
'
0 0.1 . . . 1.1
(
σijm σW
=
'
0 0.1 . . . 1.1
(
(4.9)
The length of the row matrix given in (4.9) is 12, and for the case of R = −1 valid for one alternating normal stress together with one alternating shear stress, 12 · 12 = 144 ar combinations exist. For each criterion, the value of the calculated σσW was inserted into a 12 by 12 matrix. An isoline with a value of one was then plotted using the contourfunction in MATLAB. The contourfunction automatically finds the critical combinations of stresses yielding σar by interpolation between neighbouring values in the matrix. This was deemed preferable to solving the criteriaequations, and expressing one stress component as a function of another. Especially the equations for the criticalplane criteria would have been challenging to solve.
4.8.2. Material Parameters One of the benefits of normalizing stress components with respect to σW is that they become dimensionless. The stress components σσxa and τσxya corresponding to the faW W tigue limit for combined loading may then be plotted in the same diagram, regardless of materials (diﬀerent σW ). When plotting combined fatigue limits (combinations of σσxa and τσxya ) for R = −1 in a FAD, the eﬀect of the mean stress sensitivity is W W removed for most of the fatigue criteria. For the Findley criterion however, the constant k needs to be determined based on σW , σA and τW . As the latter fatigue
28
4.9. Fatigue Database ¯ A ) and k(τW ) for the three diflimits vary between materials, the mean values k(σ ferent material groups were used. These are given in table 5.1. The resulting failure assessment diagrams are given in figure 5.2.1, 5.2.2 and 5.2.3.
4.9. Fatigue Database An extensive search for suitable fatigue tests from the literature was conducted. The search yielded a total number of 268 individual tests spanning 20 materials. It was decided to sort the data into three categories, carbon and low alloy steels, Aluminium alloys, and cast irons. Information about the collected materials and their sources are provided in table 4.1.
4.9.1. Selection Process The search was restricted to only include fatigue limits in the high cycle regime, which is here defined as 106 cycles or more. A fatigue limits/strengths for the lower ranges were ignored. All fatigue limits were reported to be conducted on either solid or hollow unnotched specimens. The majority of tests are determined by either SN testing or the staircase method, although information is lacking regarding some of them. An overview is given in table 4.1. Fatigue limits for pure uniaxial cases were included where available. Materials are gathered from what was deemed as trustworthy sources. Occasionally when the original paper cited as the primary source was unavailable, data reported in other papers by same authors as the original paper were used. These cases are marked with an asterisk * in table 4.1.
4.9.2. Determination of Missing Parameters When material parameters relevant for the fatigue assessment were unavailable, these were approximated using FKMRichtlinie. In large, this meant determining the mean stress sensitivity M and σA from equation (2.35) and (2.18), when σA was unknown. The constants utilized were gathered from table 2.1. The carbon and lowalloy steels were assumed to belong to the group einsatzstahl, while the aluminium alloy 76ST61 count as an aluminiumknetwerkstoﬀ. The two groups of cast irons were GS and GJL, with constants chosen accordingly. As previously mentioned, the M determined from FKMRichtlinie is valid for 106 cycles. Many testseries (see table A.1) were reported to apply for >106 cycles.
29
4. Procedure
Table 4.1.: List of materials collected from the literature and their references. For some materials, several data sets exist and and each individual data set is numbered with a number inside a parenthesis. Collected Primary Material Tests Remarks from source Carbon and low alloy steels 0.1%C Steel [25] XC18 Steel [21] Mild Steel [3] St35 Steel [22] St60 Steel [6] Swedish Hard Steel [3] Ck 35 V [6] C20 Annealed Steel [23] 34Cr4 (1) [22] 34Cr4 (2) [22] 34Cr4 (3) [22] 30CrMo16 (1) [24, 21] 30CrMo16 (2) [23] 25CrMo4 (1) [21] 25CrMo4 (2) [22] S65A [25] 42CrMo4 [22] 25CrMo4 (3) [6] 3.5% NiCr Steel [25] 34CrMo4 V [6]
Yes Yes No, [27] No,[28] No, [29],[30] No, [27] No, [31] No, [32] No,[33, 34, 35] No,[34, 35] No,[34, 35] Yes No,[36] No,[37] No,[37] Yes No,[38] No,[39],[40],[41] Yes No, [31]
7 5 10 12 7 12 11 3 9 14 4 16 29 4 8 27 9 12 7 15
Aluminium alloys 76ST61 (1)(3)
Yes
21
Nodular graphite cast irons “Silal” Cast Iron [20] ENGJS8002 [23]
Yes No,[42],[43]
7 4
Lamellar graphite cast irons GG30 [6] Grey Cast Iron [3]
No, [31] No, [27]
7 8
Sum:
268
[26]
* * * *
*
*
* Overlap of authors between primary source and paper the tests are collected from. ( ) Several data sets for each material exists and are numbered accordingly.
30
4.10. StressCycle From Industry Without suﬃcient information, the FKMdetermined M was assumed to be valid for these cases as well. This assumption might prove passable for steels, where the fatigue limits at higher cycles are nearly identical as the slope of an SN curve flattens out. It is not however justifiable for aluminium alloys, and a special exception was made for the alloy 76ST61. Since the uniaxial fatigue limits σW were provided for 106 , 107 and 108 cycles, diﬀerent values of M and σA were expected for each Nf . The solution was to calculate the fatigue strength coeﬃcient σf′ using the HempelMorrow line given in equation (2.17) and parameters valid for Nf = 106 . The value of σf′ was calculated to σf′ = 429.5 MPa. Since σf′ is a constant, σA for 107 and 108 cycles could be determined using equation (2.17), and M from equation (2.18).
4.10. StressCycle From Industry A fatigue assessment of a typical stresscycle from the industry was also carried out. Very little information is provided due to protection of confidenciality, and it is chiefly included here to illustrate the fatigue assessment and use of multiaxial criteria for a cycle with variableamplitude stresses in three dimensions. The stress cycle consisting of the stress components σx , σy and τxy normalized with respect to the largest absolute value of the occuring stresses σx max is given in figure 4.10.1. Selected values of the stresses occuring throughout the cycle is given in table 4.2.
Normalized Stress
Cyclic Stresses 1 0.8 0.6 0.4 0.2 0 −0.2 −0.4 −0.6 −0.8 −1 −1.2 −1.4
σx σy τxy
0
20
40
60 80 Step
100
120
140
Figure 4.10.1.: Cyclic stresses for dynamically loaded mechanical component.
31
4. Procedure Table 4.2.: Extreme values of stresses during a cycle of a dynamically loaded component. σx,max σx,min σy,max σy,min τxy,max τxy,min τxy σx max σx max σx max σx max σx max σx max σx max Value Step
0.94 23
1.00 89
0.28 23
0.28 89
0.12 53
0.38 89
0.12 23
As so little was previously known about the cycle, several assumptions were necessary in order to perform the fatigue assessment. 1. The material is assumed to be a Stahl ausser diesen with Rm = 1000 MPa and fatigue limits and other parameters calculated from FKMRichtlinie according to section 2.5. The parameters are given in table 4.3. 2. The length of the cycle is given as 142 steps. Assuming the specimen is rotat◦ ing, an angular step of 2.5◦ corresponds to 360 = 144 steps, leaving two steps 2.5◦ short of a full cycle. It is assumed that the two missing steps do not impact the fatigue assessment. This is supported by the fact that the stresses in step 1 and 142 are close to each other, and relatively far from any influencing global extremevalues. 3. When using the ASMEmethod, it was assumed that each step corresponds to a point in time with equal diﬀerence between two consecutive values. The ASMEmethod is then used by substituting points in time with steps. The HempelMorrow line given in (2.17) was used to determine σA . The resulting material parameters and fatigue limits are given in table 4.3. Table 4.3.: Material parameters for a constructed steel according to FKMRichtlinie and assumed to be valid for the stress cycle given in figure (4.10.1). Rm σW τW σA M k(σA ) k(τW ) (MPa) (MPa) (MPa) (MPa) 1000
32
450
259.7
360
0.250
0.237
0.156
5. Results 5.1. Determination of Parameters The calculated parameters are for comparisons sake given together with the reported material parameters in table 3.1 for carbon/low alloy steels and table 3.2 for Aluminium/cast irons. The degree of appropriateness can to a certain degree be determined by comparing the calculated σA with the reported value in cases where this was obtainable. In general, the σA calculated from FKMRichtlinie and the HempelMorrow line is larger than the reported value. In this respect, FKM and HempelMorrow yield nonconservative results. It is worth noting however, that the true experimentally determined σA was only reported for about half of the test series used in the fatigue assessment. Average values for the material parameters M, k(σA ) and k(τW ) used in the fatigue assessment are given for the three material groups in table 5.1.
Table 5.1.: Average values of M, k(σA ) and k(τW ) reported in table 3.1 and 3.2 with respect to material grouping. Only values used in the fatigue analysis was counted in. Material group Carbon and low alloy steels Aluminium Cast irons
M
k(σA )
k(τW )
0.204 0.431 0.366
0.194 0.427 0.362
0.263 0.303 1.286
Comparing the average values, the Findley constant k determined with the fatigue limits σW and σA lie close to the mean stress sensitivity. There are however a notable diﬀerence between the mean values k(σA ) and k(τW ) between material groups.
33
5. Results
5.2. Failure Assessment Diagrams As previously stated, a failure assessment diagram is a visual presentation of a criterion at the fatigue limit. The area under each individual curve represents the safe combinations, where a criterion does not predict failure. Three such diagrams are presented here, with the criteria calculated using the average values for each material group given in table 5.1. The criteria are plotted for fully reversed R = −1 stresses, with no phase diﬀerence, αij = 0◦ . Since no meanstresses are present, the influence of M is negated. For the sake of comparison, Findley evaluated with k(σA ) is left out. Only criteria assessed the traditional way are plotted. Fatigue test data for the corresponding cases and shear and normalstresses are plotted for each material group as well. For the case of uniaxial stresses, only the shear stresses are plotted (points along the τσxya axis). Since the criteria are W calculated based on average material parameters, some deviation between the points and the curves is expected. The FAD for all three material groups are given in table 5.2.15.2.3. Some general trends are immediately valid for all material groups. Only the Findley criterion is shown to adapt to the change between fatiguefracture governed by either normal or shearstresses, due to k being evaluated by σW and τW . All the other criteria are the same for all material groups. The TrescaSines criterion is identical to the ASMEcriterion, and due to this overlap, the ASMEcriterion is the only one shown. The normal stress criterion, which only takes normalstresses into account predicts a limiting state of nonfracture both at pure shear τσxya = 1 and for pure normal stress W σxa = 1. For fully reversed loading, this is easily explained using principal stresses σW (equation (2.13)) and it can be shown that the largest alternating amplitude is 5 2 allowed to be equal to σW . The same goes for pure shear stress, as σ1 = τxya = σW . 5 2 = σ , The MisesSines criteria predicts for fully reversed normal stress σar = σxa W 5 2 τxya 1 √ and fully reversed shear stress, σar = 3τxya =⇒ σW = 3 = 0.577. The TrescaSines criterion predicts σar = 2τxya =⇒ τσxya = 12 = 0.5 for pure shear, and σar = W 2τxya = 2 · 12 σ1,max =⇒ σσxa = 1 for pure normal stress. The end points for the Findley W criterion are challenging to show in a practical manner due to the criticalplane. For carbon and low alloy steels plotted in figure 5.2.1, the fatigue test data seem to lie in the vicinity of the shear stress criteria. The predictions for these seem overall to be conservative, while the normalstress criterion is mainly nonconservative. As for the carbon and low alloy steels, the fatigue data for aluminium plotted in figure 5.2.2 show a good correlation with the shear criteria. The FAD for cast irons
34
5.3. Predictions for Tests at the Fatigue Limit
Criteria and tests for carbon/low alloy steels.
1
τxya / σW
0.8
Normal Stress Mises−Sines Tresca−Sines ASME
0.6
Findley (τW) Test Data
0.4 0.2 0
0
0.2
0.4 0.6 0.8 σxa / σW
1
Figure 5.2.1.: Failure assessment diagram, R = −1 and αij = 0◦ . Test data are 34 fatigue tests for carbon/low alloy steels. given in 5.2.3 show data in good correlation with the normal stress criterion, rather than with the shear stress criteria. Some outliers are present.
5.3. Predictions for Tests at the Fatigue Limit What follows are the results from the evaluation of the fatigue criteria at the collected tests from the literature. An overview of the data is given in table 3.1 and 3.2, while the data themselves are given in appendix A, tables A.2 to A.11. The predictions for all 268 tests provided in table 5.2 includes all loading cases present. The outcome is also plotted in the histograms 5.3.1 and 5.3.2. The fatigue tests were grouped according to selected stress states and materials. Both predictions based on traditional criteria and ASMEcriteria are presented side by side for the sake of comparison. The predictions are given in table 5.2 and 5.3.
5.3.1. Predictions for Selected Loading Cases Predictions for several selected stress ratios and variations of loading parameters are given in table 5.2 and 3.1.
35
5. Results
Criteria and tests for aluminium 76S−T61.
1
τxya / σW
0.8
Normal Stress Mises−Sines Tresca−Sines ASME
0.6
Findley (τW) Test Data
0.4 0.2 0
0
0.2
0.4 0.6 0.8 σxa / σW
1
Figure 5.2.2.: Failure assessment diagram, R = −1 and αij = 0◦ . Test data are 13 fatigue tests for 76ST61.
Criteria and tests for cast irons.
1
τxya / σW
0.8
Normal Stress Mises−Sines Tresca−Sines ASME
0.6
Findley (τW) Test Data
0.4 0.2 0
0
0.2
0.4 0.6 0.8 σxa / σW
1
Figure 5.2.3.: Failure assessment diagram, R = −1 and αij = 0◦ . Test data are 12 fatigue tests for cast irons.
36
5.3. Predictions for Tests at the Fatigue Limit The normalstress criterion is the only criterion with overall nonconservative prear dictions, as the mean value of σσW lies beneath 1. The criterion performs quite badly when used to assess the 11 tests for fully reversed shear stresses. The standard deviation sp = 0.14 is lower or equal than the standard deviations for other criteria. This indicates that the predictions are gathered relatively close. For the normal stress criterion, no overall diﬀerence is found when comparing the ASMEassessment method with the traditional critical plane approach. The MisesSines criterion yields good predictions overall, with predictions slightly on the conservative side. For fully reversed loading with αxy ̸= 0◦ , MisesSinesASME yields a mean value beneath 1. For loading with mean stresses without a phase shift, a mp very close to one is observed for both MisesSines and MisesSinesASME. The sp however is quite high. The TrescaSines criterion has one of the overall largest spread with sp = 0.22 and sp = 0.21 for TrescaSinesASME. Both versions provide highly inaccurate predictions for the pure shear tests. For stresses with R = −1 and αxy ̸= 0◦ , a large spread in the predictions for both variations of the criterion is observed. The mean value however is very good for TrescaSines. The ASMEcriterion stands out with a accurate mean value mp = 0.99. The standard deviation is however quite large signalling a large spread in predictions. For the 11 cases of pure shear, the predictions are highly conservative and inaccurate (large spread). For cases with mean stresses present, the criterion is nonconservative. For stresses with R = −1 the ASMEcriterion yields the same predictions as TrescaSines. The Findley criterion shows an improvement in mean value mp when assessed with the ASMEmethod. This is especially prominent for stresses where R ̸= −1 without phase shifts. The Findley criterion using k(σA ) yields overall a mp slightly closer to one than when using k(τW ), but the latter performs extremely well for the 11 pure sheartests. A distinct decrease in mean value occur for FindleyASME and R ̸= −1, αxy ̸= 0◦ . For cases given in table 3.1 where σy is taken into account, the predictions for all criteria are generally characterized by a large spread in predictions. The normal stress criterion however, yields similar predictions for a shear stress component with both one and two normal stress components present. The MisesSines criterion yields very good predictions, but the results worsen when assessed with the ASMEmethod. For cases with three stress components, the Findley criterion yields nonconservative predictions with a high degree of spread.
37
5. Results
Number of Tests
Normal Stress Criterion 70 60 50 40 30 20 10 0 0.2 0.4 0.6 0.8
2*sp mp
1
1.2 1.4 1.6 1.8 σar / σW
2
2.2
(a)
Number of Tests
Mises−Sines Criterion 70 60 50 40 30 20 10 0 0.2 0.4 0.6 0.8
2*sp mp
1
1.2 1.4 1.6 1.8 σar / σW
2
2.2
(b)
Number of Tests
Tresca−Sines Criterion 70 60 50 40 30 20 10 0 0.2 0.4 0.6 0.8
2*sp mp
1
1.2 1.4 1.6 1.8 σar / σW
2
2.2
(c)
Figure 5.3.1.: Predictions and their distribution for the criteria normal stress, MisesSines and TrescaSines for all 268 tests.
38
5.3. Predictions for Tests at the Fatigue Limit
Number of Tests
ASME Criterion 70 60 50 40 30 20 10 0 0.2 0.4 0.6 0.8
2*sp mp
1
1.2 1.4 1.6 1.8 σar / σW
2
2.2
(a)
Findley (σ ) Criterion Number of Tests
A
70 60 50 40 30 20 10 0 0.2 0.4 0.6 0.8
2*sp mp
1
1.2 1.4 1.6 1.8 σar / σW
2
2.2
(b)
Number of Tests
Findley (τW) Criterion 70 60 50 40 30 20 10 0 0.2 0.4 0.6 0.8
2*sp mp
1
1.2 1.4 1.6 1.8 σar / σW
2
2.2
(c)
Figure 5.3.2.: Histograms of all predictions from the ASME criterion and Findley k(σA ) and k(τW ) for 268 tests.
39
5. Results From figure 5.3.1 and 5.3.2, it is apparent that outliers are present. For the normal stress criterion, the outliers on the conservative side are caused by the aluminium alloy 76ST61, test nr 227 and 235. Large mean stresses for σx are present in both tests. Compared to the other criteria, the predictions are closely gathered on the nonconservative side. Some testseries seem to be the cause of outliers for many criteria, namely 34CrMo4 V. This testseries yields outliers for MisesSines, TrescaSines, ASME and both variations of Findley. Test nr 212 with τxym = 794.6 MPa causes the most nonconservative prediction for both Sinescriteria and the ASMEcriterion. TrescaSines and the ASMEcriterion produce low quality predictions for cast iron from Nishihara/Kawamoto, and these cause the conservative outliers seen in the histograms.
5.3.2. Comparison of Predictions for Material Groups The materials were grouped into three distinct material divisions: carbon and low alloy steels, aluminium alloys and cast irons. A summary of the predictions are given in table 3.1. The group with carbon and low alloy steels is by far the largest, consisting of 221 experiments (≈ 82.5% of all tests). The normal stress criterion yields nonconservative predictions for all material groups, but more for the carbon/low alloy steels and aluminium 76ST61. An acceptable degree of accuracy is noticeable for the predictions regarding cast irons. The traditional assessment method and the ASMEassessment method provide no diﬀerences in predictions. MisesSines and MisesSinesASME yield quite similar predictions, with a mean value closer to one for the latter. A high degree of spread is observed for cast irons. TrescaSines provide a quite large spread in predictions for all three material groups, and the meanvalue is closer to 1 for the carbon/low alloy steels than aluminium and cast irons. The ASMEcriterion predictions have a slightly nonconservative mean value for carbon and low alloy steels, but a large spread. For both the aluminium tests and cast irons, the mean value is conservative. Predictions for cast iron are marked by high spread and are thus inaccurate. The Findley criterion shows an improvement in mean value for carbon and low alloy steels, and cast irons, when assessed with the ASMEmethod. This is especially pronounced for Findley (σA ) and carbon/low alloy steels. Predictions made with Findley (τW )ASME are betterm but still contains a high degreee of spread.
40
1.38 ± 0.28
1.04 ± 0.03 1.04 ± 0.03 1.02 ± 0.08 0.92 ± 0.11 1.23 ± 0.24 1.10 ± 0.20
One normal stress and one shear component present, R=1, αxy = 0◦ , 48 tests in total. Prop. method 0.93 ± 0.08 1.06 ± 0.08 1.14 ± 0.12 1.06 ± 0.08 ASMEmethod 0.93 ± 0.08 1.06 ± 0.08 1.14 ± 0.11 1.14 ± 0.12 1.06 ± 0.08
One normal stress and one shear component present, R=1, αxy ̸= 0◦ , 33 tests in total. Prop. Meth 0.81 ± 0.12 1.09 ± 0.14 1.00 ± 0.20 1.03 ± 0.13 ASMEmethod 0.81 ± 0.12 0.93 ± 0.16 1.02 ± 0.20 1.00 ± 0.20 0.94 ± 0.13
One normal stress and one shear component present, R̸=1, αxy = 0◦ , 26 tests in total. Prop. method 0.95 ± 0.19 1.01 ± 0.19 1.07 ± 0.21 1.16 ± 0.13 ASMEmethod 0.95 ± 0.19 1.01 ± 0.19 1.07 ± 0.21 0.89 ± 0.19 1.04 ± 0.16
1.10 ± 0.18 1.03 ± 0.17 1.03 ± 0.04 1.03 ± 0.04
1.09 ± 0.14 1.02 ± 0.15 1.12 ± 0.21 1.12 ± 0.21
1.38 ± 0.28 1.38 ± 0.28
Pure shear, R=1, 11 tests in total. Prop. method 0.69 ± 0.14 ASMEmethod 0.69 ± 0.14 1.20 ± 0.24 1.20 ± 0.24
0.99 ± 0.23
All 268 tests regardless of stress ratio or stress components. Prop. method 0.88 ± 0.14 1.04 ± 0.15 1.08 ± 0.22 ASMEmethod 0.88 ± 0.14 1.02 ± 0.16 1.09 ± 0.21
Table 5.2.: Comparison of predictions for all criteria and diﬀerent loading cases. The predictions are presented as the mean value plus/minus one standard deviation, mp ± sp . Criterion Assessment Method Normal Stress MisesSines TrescaSines ASME Findley (σA ) Findley (τW )
5.3. Predictions for Tests at the Fatigue Limit
41
5. Results
Normal Stress
MisesSines
Criterion TrescaSines ASME
Findley (σA ) Findley (τW )
Table 5.3.: Comparison of predictions for all criteria, a selection of stress components present, and diﬀerent groups of materials. No selection of stressratios or the like have been made. The predictions are presented as the mean value plus/minus one standard deviation, mp ± sp . Assessment Method
Aluminium 76ST61. 21 tests in total, nr. 222242. Prop. method 0.92 ± 0.19 1.06 ± 0.11 ASMEmethod 0.92 ± 0.19 1.06 ± 0.11
1.11 ± 0.40 1.11 ± 0.40
1.14 ± 0.13 1.14 ± 0.13
Carbon and low alloy steels. 221 tests in total, nr. 1221. Prop. method 0.86 ± 0.14 1.03 ± 0.12 1.07 ± 0.20 ASMEmethod 0.86 ± 0.14 1.01 ± 0.13 1.08 ± 0.19
1.09 ± 0.40
1.07 ± 0.14
0.97 ± 0.20
1.19 ± 0.18 1.06 ± 0.21
1.02 ± 0.13 1.02 ± 0.13
1.08 ± 0.13 1.01 ± 0.15
Two normal stress components regardless of stress ratio and phase shift, 19 tests in total. Prop. method 0.83 ± 0.10 0.91 ± 0.14 0.96 ± 0.35 0.92 ± 0.21 ASMEmethod 0.83 ± 0.10 1.04 ± 0.12 1.02 ± 0.27 0.81 ± 0.14 0.89 ± 0.19
1.17 ± 0.21 1.11 ± 0.15
1.03 ± 0.08 1.03 ± 0.08
1.10 ± 0.18 1.03 ± 0.17
0.92 ± 0.22 0.88 ± 0.20
Ttwo normal and one shear stress component regardless of stress ratio and phase shift, 18 tests in total. Prop. method 0.84 ± 0.12 1.01 ± 0.08 1.10 ± 0.21 1.07 ± 0.14 1.18 ± 0.18 ASMEmethod 0.84 ± 0.12 1.06 ± 0.15 1.11 ± 0.21 0.86 ± 0.21 1.01 ± 0.14 1.10 ± 0.16
Cast Irons, 26 tests in total, nr. 243268. Prop. method 0.97 ± 0.08 1.07 ± 0.33 ASMEmethod 0.97 ± 0.08 1.04 ± 0.32
42
5.4. StressCycle of Dynamically Loaded Component
5.4. StressCycle of Dynamically Loaded Component The results of the fatigue assessment for the dynamically loaded component with stresses plotted in figure 4.10.1 are given in table 5.5. All stressvalues are normalized with respect to σx max . The stress cycle was evaluated using all criteria and both assessment methods. The conversion given in equation 5.1 gives the equivalent uniaxial amplitude normalized with respect to σW . Values for the stress cycle normalized on σW are given in table x. σar σar σx max = · (5.1) σW σx max σW All predictions σxσarmax are below 1, and so with the assumption that σx max < σW for the real material (not the approximated σW = 450 MPa), failure is not predicted. For the normal stress criterion, the proportional assessment method and ASMEmethod yield no diﬀerences in predictions. The critical plane is unchanged between the two, and the stresses which result in the largest σxσarmax occur on the same steps. It is noticeable that the critical plane is “chosen” based on the highest combination of normal stresses, as the shear stress occurring on the same plane and the resulting shear stress amplitude is lower than those for the shear stress criteria. For the MisesSines criterion, the variation MisesSinesASME yield a more conservative value, but the stress values σij used in the assessment of the criteria are all taken from the same steps. The TrescaSines and TrescaSinesMises criterion show diﬀerences in the critical plane, as well as a marginal diﬀerence in σxσarmax . The values however are taken from the same steps. The ASMEcriterion yields the same σxσarmax as TrescaSinesASME. Both criteria regardless of assessment method (for SinesMises criterion) yield the most nonconservative predictions out of all the fatigue criteria. The Findley criterion for both k(σA ) and k(τW ) yield identical results, but marginally diﬀerent critical planes. Figure 5.4.1 show the stresses on the predicted critical planes for the normal stress criterion, TrescaSines and the Findley (σA ) criterion throughout the cycle. For the normal stress criterion, the plane is chosen based on the normal mean and amplitude stress. This is visible in 5.4.1 (a). The Findley (σA ) criterion finds the critical plane based on shear stress amplitude and maximum occuring normal stress. Compared to
43
5. Results Table 5.4.: Results of stresscycle assessment for all criteria and both assessment methods normalized with σW . Normal Stress
MisesSines
TrescaSines ASME
Fin. (σA ) Fin. (τW )
Proportional assessment method σar 0.44 0.43 σW
0.33

0.41
0.39
ASMEmethod σar 0.44 σW
0.33
0.33
0.41
0.39
0.40
the critical plane predicted by the normal stress criterion, the variation in parameters taken into account for each criterion becomes apparent. Figure 5.4.1 also show at which step the extreme values of stresses on the diﬀerent critical planes occur. This coincides well with the steps given in table 5.5.
44
5.4. StressCycle of Dynamically Loaded Component
Table 5.5.: Results of stresscycle assessment for all criteria and both assessment methods. The names for the criteria are shortened, so that NS corresponds to the normal stress criterion etc. NS
MS
TS
ASME
Proportional assessment method σar 0.97 0.96 σx max
0.73

0.90
0.86
φ (◦ )
6

56

150
149

0.87
0.86
23
23
(0.49)
(0.48)
89
89
0.23
0.24
23
23
0.50
0.49
89
89
σmax (φ) σx max
Value
0.91

(0.38)
Step
23

23
σmin (φ) σx max
Value
1.07

(0.86)
Step
89
τmax (φ) σx max
Value
(0.10)
Step
54
τmin (φ) σx max
Value (0.30) Step
F (σA ) F (τW )

89 
0.47

89 
76
0.27

23
ASMEmethod σar σx max
0.97
0.89
0.74
0.74
0.90
0.86
φ (◦ )
6

146

150
149
Interval
2389
2389
2389
2389
2389
2389
() Stress values in paranthesis not used by the criterion.
45
5. Results
Normalized Stress
Normal Stress Criterion 1.2 1 0.8 0.6 0.4 0.2 0 −0.2 −0.4 −0.6 −0.8 −1 −1.2 −1.4
σ(φ) τ(φ)
0
20
40
60
80 Step (a)
100
120
140
Normalized Stress
Tresca−Sines Criterion 1.2 1 0.8 0.6 0.4 0.2 0 −0.2 −0.4 −0.6 −0.8 −1 −1.2 −1.4
σ(φ) τ(φ)
0
20
40
60
80 Step (b)
100
120
140
Normalized Stress
Findley (σA) Criterion 1.2 1 0.8 0.6 0.4 0.2 0 −0.2 −0.4 −0.6 −0.8 −1 −1.2 −1.4
σ(φ) τ(φ)
0
20
40
60
80 Step (c)
100
120
140
Figure 5.4.1.: Stresses throughout the cycle on critical planes predicted by the criticalplane criteria.
46
6. Discussion 6.1. Requirements of a Fatigue Criterion The fatigue criteria are reviewed based on three requirements. In search for the perfect fatigue criterion, these requirements should all be fulfilled. 1. Accuracy of predictions 2. Criterion should be based on physical properties proven to have an eﬀect on fatigue damage mechanisms 3. Ease of use and implementation of criterion A good criterion should produce accurate predictions for a wide selection of materials and loading cases. Parameters such as angular frequency, phase shift and Rratios should all be correctly accounted for. The normalized fatigue prediction parameters σar given in table 5.2 and 5.3 are a quantitative measure of the accuracy of each σW criterion. The criteria are assessed based on their usability and ease of implementation. The practicing engineer is taken into account on this point. If the criterion is diﬃcult to utilize, its general accept in the engineering community will probably suﬀer as a result. Every criterion should as well be based on logical and proven material dependencies. As cumulative fatigue damage is a process involving many variables, such parameters should be taken into account as are proven to have an eﬀect on fatigue life. Hence, a perfect criterion is one which is based on proven and logical material dependencies, which gives excellent predictions, and is simple to use and implement. In reality, these three requirements might be extremely diﬃcult to fulfil. They do however provide a platform on which to compare and evaluate each criterion. The last two requirements might suﬀer from subjective opinions. With the increased availability of fatigue postprocessors, the second requirement can be questioned. The literature commonly focus on accuracy of predictions, without thought to practicing
47
6. Discussion engineers. A tradeoﬀ between these three requirements is generally the criterion which will see the most widespread use.
6.2. Assessment and Suitability of Criteria An accurate prediction is as previously stated when the equivalent uniaxial stress amplitude σar coincides with the uniaxial fully reversed fatigue limit σW . As a certain degree of scatter is expected in fatigue tests, the overall, mean value of predictions serve as a quantitative measure of the predictability of a criterion. The predictability is presented as the mean value of predictions plus/minus the sample standard deviation, mp ± sp . A high degree of accuracy is then characterized by mp close to one, and sp close to zero. It is important that the two are compared together. One might argue that a low spread is preferable to a perfect mean value equal to 1, as the mean value can be countered by introducing a fitting safety factor.
6.2.1. Normal Stress Criterion The normal stress criterion show overall inaccurate and nonconservative predictions for materials, where failure is expected to occur based on shearstress induced fatigue cracks. The results for brittle materials with a στW ratio close to 1 are however W significally better, and the predictions are far better than the shearstress criteria. The physical relevance of the criterion is well established for uniaxial, proportional cases as it is based on the HempelMorrow line. Out of the criticalplane criteria, the normal stress criterion is by far the easiest to use when utilizing the proportional assessment method. This is due to the material parameters needed for the fatigue assessment only being the mean stress sensitivity M and the fatigue limit σW . In addition, only the normalstress on the critical plane is taken into account, making calculations easier. When combined with the ASMEmethod, no diﬀerences in predictability were found. This is possibly due to the fact that only the normal stress component on the plane is taken into account, but this is further discussed in section 6.3. The computational diﬃculty is however increased whenever the ASMEmethod is used, and since no diﬀerences in predictability were found for the normal stress criterion, this should be taken into account when using the criterion.
48
6.2. Assessment and Suitability of Criteria
6.2.2. MisesSines Criterion The MisesSines criterion yields good predictions for proportional cases when assessed with the proportionalmethod. For sheardominated cases however, the criterion might be expected to yield inaccurate predictions. The validity of stress invariants may be questioned for stress histories of a nonproportional nature, but comparing the predictions for both the proportionalmethod and the ASMEmethod show that they are fairly close to each other. The predictions yielded when using the latter method are only slightly better for MisesSinesASME, but the decrease in computability is distinct. Still, the mean value of predictions for MisesSinesASME is very accurate, on par with the Findley criterion. Since it is based on stressinvariants rather than criticalplane methodology, the implementation of MisesSines is fairly simple. The criterion is also based on empirical data for proportional loading.
6.2.3. TrescaSines Criterion The TrescaSines criterion is, together with the normal stress criterion, fairly simple to use. The criticalplane is relatvely easy to determine, since it is determined by the maximum shear stress amplitude. Utilizing the stressinvariant for mean stresses, the fatigue assessment as a whole is relatively simple. The predictions however, are marked by a high degree of spread, especially for brittle materials such as cast irons. The predictions for TrescaSinesASME are somewhat similar overall, and thus the ASMEmethod only contributes negatively in terms of computationability.
6.2.4. ASMECriterion The ASMEcriterion, while not modified for mean stresses yield (not surprisingly) inaccurate predictions with a high degree of spread. The good mean value of X for all of the 268 fatigue tests is a result of pure chance, as the more diﬀerentiated stress cases show. For stresses with ratio R = −1 , the predictions are equal to the TrescaSines criterion. This gives grounds to the validity of the approximation σeq,T,a ≈ 2τa,max (ASM E). The criterion itself is somewhat easier to compute than the criticalplane criteria, not requiring to calculate stresses on every plane φ ∈ [ 0◦ , 180◦ ] , and provided the extremevalues and their points in time are known. When these points in time are unknown, the computability decreases.
49
6. Discussion
6.2.5. Findley Criterion The Findley criterion is the most extensive criterion to compute and implement. It requires the determination of k, here only shown for pure shear or pure normal stresses and the stress ratios R = −1 and R = 0 in equation (2.28). Since the fatigue limits used to determine k yield diﬀerent values, the notion of k as a constant should be addressed. Since the k have such a large impact on the accuracy of predictions, the uncertainty of which two fatigue limits should be combined increases insecurity around the implementation. In this thesis, two k ’s were evaluated with σW in combination with σA and τW . From table 5.2 the diﬀerence in predictions for k(σA ) and k(τW ) are apparent. Overall, the predictions when k(σA ) is used are more accurate, with a mean value closer to 1 and slightly lesser spread than for k(τW ). For fully reversed, pure shear stresses the predictions with k(τW ) are considerably better than the k(σA ). This might indicate that for stress cycles dominated by shearstresses, k should be determined using the shear fatigue limit τW , and the opposite is valid for cycles where normalstresses dominate. As a criticalplane criterion, it makes use of both the shear and normalstress on the critical plane. This makes the calculation slightly more challenging than the other critical plane criteria reviewed here, as they all only utilize one stress component (either the shear stress or normal stress). The eﬀect is however diminishing when using computational resources like MATLAB. A significant improvement of the mean value of predictions is observed when using the ASMEmethod, although the usability of the criterion is diminished. Not only are the stresses for each stress component on the plane assessed together with the stresses at every other point in time calculated, but this has to be done for φ ∈ [ 0◦ , 180◦ ] .
6.3. Proportional Method vs ASMEMethod Fatigue criteria derived for proportional loading are commonly used to assess situations where the loading is nonproportional. The common method of determining stress parameters and subsequently the criteria, is here called the proportionalmethod and explained in section 4.5. According to the proportional method, global extreme values should be used to determine relevant stress components used by the fatigue criterion. The alternating and mean stress components may then be found by equation (2.10) and (2.11). For nonproportional loading however, the stressvalues utilized by a criterion may occur at potentially large diﬀerences in time. An example of such a stress cycle
50
6.3. Proportional Method vs ASMEMethod is presented in figure 6.3.1, and the question can be raised of the validity of the proportional method for such cases. Assuming that the plane on which the stresses in figure 6.3.1 are working, is the critical plane for both the normal stress criterion and the Findley criterion. This assumption is only done here to explain the advantages of the ASMEmethod. The proportional method of determining stress values, will yield the maximum shear stress amplitude on the plane as τa (φ) = 12 [τ (φ, t1 ) − τ (φ, t1 )]. The shear stresses occurring at the points in time t1 and t2 are used. The normal stress amplitude may be determined as σa (φ) = 12 [σ(φ, t3 ) − σ(φ, t1 )] = 12 [σ(φ, t3 ) − σ(φ, t2 )], as the normal stress occurring at t1 and t2 are equal. The mean stress components are determined accordingly. The normal stress criterion makes use of both σa (φ) and σm (φ), while the shear stress components on the plane are disregarded. The normal stresses occurring in the relative vicinity of t3 then govern the predictions made by the criterion. The Findley criterion utilizes both τa (φ) and σmax (φ), and while the largest τa (φ) is found around t1 and t2 , the maximum normal stress occurs at t3 . Since t3 ≫ t1 , t2 it is not obvious how the normal stress may have a direct, physical influence on the fatigue damage. This aspect is however neglected when using the proportional method. The determined stressvalues are used indiscriminately, only in capacity of occurring on the same plane throughout the cycle.
σ(φ), τ (φ)
σ(φ) τ (φ) .
t 1 t2
t
t3
Figure 6.3.1.: Stress cycle with one shear and one normal stress component. The proposed ASMEmethod attempts to remedy this by using stresscomponents calculated on intervals between two points in time, where the stresses are hypothesized to have a specific relevance to each other. Stress components for an interval [tˆ, t] are then based only on the stresses occurring at time tˆ and t. When following the ASMEmethod, each stress component at each point in time, is compared relative to every other stress component, occurring at every other point in time. The
51 1
6. Discussion maximum and minimum values on each interval are used to find amplitudes and mean stresses, and so each fatigue criterion may be calculated intervalwise. The interval in time which corresponds to the largest predicted σar then governs fatigue damage on the plane. For the cyclic stresses in figure 6.3.1, the intervals [t1 , t3 ] and [t2 , t3 ] yield the same amplitude and mean normal stress. When using the ASMEmethod, the normal stress criterion then predicts the same local σar for both intervals. For interval [t1 , t2 ], the amplitude σa (φ) = 0, which will yield a smaller σar only based on σm (φ). For the Findley criterion in combination with the ASMEmethod, the interval [t1 , t2 ] yields the largest shear stress amplitude, but a σmax (φ) = σ(φ, t1 ) = σ(φ, t2 ). The interval [t1 , t3 ] yields a smaller shear stress amplitude, but a significantly larger maximum normal stress. The interval [t2 , t3 ] yields the same values as for [t1 , t3 ], with exception of a negative τm (φ). The mean shear stress is however not taken into account by the Findley criterion. The influence of this assessment method is larger for the Findley criterion, and in a positive way (see section 5.3). This might be caused by the fact that both normal and shear stresses are taken into account. For the normal stress criterion however, the ASMEmethod were in this case reduced to a laborious alternative for determining the amplitude and mean normal stress. The ASMEmethod then shows promise, and deserves further testing. This is especially for criticalplane criteria where both normal and shear stresses are taken into account.
6.4. Fatigue Assessment of Stress Cycle An interesting aspect when comparing the results from the fatigue database with the results for the stress cycle, is the relative diﬀerences between the criteria predictions. Based on the trend from the fatigue tests as shown in the failure assessment diagrams, the normal stress criterion should yield a more nonconservative prediction than the other criteria for most combinations of shear and normal stresses. In ar that respect, the σσW predicted by the normal stress criterion should be below the σar values for the criteria based on shear stress. It is however above these values, σW which is intriguing. The summaries are mainly done for combinations of one normal stress together with a shear stress, and do not provide suﬃcient information on cases where two normal stresses are present. The low value of φcrit also show that the critical plane is quite close to the xaxis, which indicates that the fatigue assessment is dominated by the quite large σxσxmax component. Assuming the fatigue assessment 52
6.5. A Note on the Availability of Fatigue TestData is dominated by the σxσxmax component, which might be a more than reasonable assumption, this would correspond to the bottom right corner of a fatigue assessment ar diagram. The overall similarity of the the σσW values support this. The ASMEcriterion however stands out as the most nonconservative. Since it does not take mean stresses into account, this is reasonable, as the other criteria account for mean stresses and are expected to yield predictions closer to failure on the conservative side.
6.5. A Note on the Availability of Fatigue TestData This thesis builds on a now long tradition of comparing multiaxial fatigue criteria with tests found in the literature. In this regard it falls in line with several works based on the same basic pattern. Older criteria are compared with a newly proposed criterion or assessment method, using limited test data collected from the literature, often from unreliable sources. It is clear that the topic of fatigue test data for proportional and nonproportional data deserves to be discussed further. As table 4.1 shows, an extensive search after usable and trustworthy experimental results was conducted. Gathering such experimental data proved to be a long, and often frustrating process, during which several concerns was discovered. The availability of readily usable fatigue test results is a major issue. Countless experiments have been performed, but several authors only publish the results and are content with referring to the test data used. In the rare case that the test data are presented, it is often in the form of graphs that require a potential inaccurate reading in order to become usable. Several citations are also lacking in accuracy, as they occasionally hail nonprimary sources as the origin of the data. With the apparent demand of usable experimental data, researchers are forced to carry out own investigations or make do with tests provided in the literature. As so few new experiments are published, most of the available data stem from relatively old sources. The test series performed by Nishihara & Kawamoto [27], Lempp [38], Zenner et al. [35, 33] and Froustey & Lasserre [24] are among the most frequently cited. This in itself is problematic for a number of reasons. The Nishihara & Kawamoto data were published in Japan in 1945. The original Japanese paper is extremely hard to procure, as well as any translated versions. The amount if use seems in no way to be aﬀected by the elusiveness of the original publication. With no copy of the original source available, great caution should be exercised with respect
53
6. Discussion to the quality and aptitude of these investigations. Information on how the tests were conducted is lost, assumptions are unknown, testing apparatus is uncertain and so on. This leaves the user to trust in secondary sources at best when searching for data suitable for validating purposes. Of the roughly 30 papers reviewed in connection with this thesis, the Nishihara & Kawamoto data is referred to in 12 of them. It is questionable as well that such a large amount of later investigations are relying on experiments from the same source. New and proposed criteria are constantly being tried against the same experiments. The lack of new input can have a severe impact if this trend continues. This thesis is no exception, as all the examples mentioned are included and used here. This is the result of a tradeoﬀ between need and resources. The need and wish for as many tests as possible to be able to provide an indepth statistical evaluation of predictions, against the urge to only employ safe original sources and up to date experiments. Several private databases containing fatigue experiments are known to exist, and are used to great eﬀect by their assemblers. Most notably are the databases by Papuga and Susmel [44]. In an attempt to remedy this, Papuga has amassed a large amount of fatigue tests from the literature on his webpage [5]. These data are available to the public, and provide an excellent starting point for further investigations. One can only speculate on the reasons why so few new experiments are being published. Since up to date experimental data are so scarce, new and fresh experimental data would surely receive a lot of attention.
6.6. Continued Work and Suggested Improvements When comparing the work done in this thesis with the quite extensive problem description, it becomes apparent that only a portion is covered here. In addition to explore the topics not included here, some ideas for further investigation also emerged as a result of the investigation.
Expansion of the fatigue database Due to the lack of test data, it would be desirable to perform inhouse fatigue testing of select materials. Not only would they serve as a trustworthy platform for future investigations, but would surely attract the attention to any papers they are published in. A further expansion of the existing testdatabase with experimental data from the literature should be
54
6.6. Continued Work and Suggested Improvements considered as well. Especially the sections regarding aluminium alloys and cast irons should be improved in order to give statistically suﬃcient results. More criteria combined with the ASMEmethod A total of 11 diﬀerent versions of wellknown fatigue criteria were examined during this investigation. The FindleyASME criterion stands out, with an overall increase in accuracy compared to the traditional Findley criterion. The ASMEmethod of assessing stress cycles shows promise and deserves to be further tested on other criteria. Improved calculation scripts and database management systems All of the main calculations in this thesis were done in MATLAB, while the literature tests were gathered and stored in Excel. They were chosen at the time out of practicality and previous experience. While the MATLABExcel setup performed suitably well, there is some room for improvement. The storing of data in Excel works fine for a limited amount of data. As the amount increases, management of the data becomes increasingly hard to handle. Large Excelsheets are also prone to accidental misentries, where faulty values may go unnoticed. The scripts used to perform the fatigue assessment were all made by the author. In no way should they be considered as optimal in terms of computational elegance and optimization. This should not have an eﬀect on the results, but will provide scripts that run smoother. In that regard, input should be sought from someone with extended computational experience. Other programminglanguages such as Python should also be considered. As the fatigue database is expanded, other options for storing the data should be considered. Available possibilities are dedicated database management systems such as MySQL.
55
7. Conclusion The main purpose of this thesis was to provide a critical review of the fatigue assessment of components subjected to nonproportional stress histories. A large database consisting of 268 biaxial fatigue limits for combined loading, spanning 27 test series and 20 materials was assembled. For the sake of comparison, cases for both proportional and nonproportional loading were included. Gathering experimental data from credible sources proved to be an exhausting process. Several comprehensive databases of the sort are known to exist, but are not, with the exception of occasionally republished snippets, readily available to the fatigue community at large. As a result, engineers and scientists are forced to make the best out of old experiments from sources of often uncertain quality. A total of 268 experimental tests were gathered in this thesis in an attempt to remedy this, which in this context can be seen as formidable. The experimental data, some of it very old, are still commonly used for validating purposes. With this in mind they have been reproduced here. The experimental data was evaluated using five criteria intended for multiaxial fatigue assessment. The original criteria included in the assessment were the normal stress criterion, Sines criterion with the von Mises stress amplitude, Sines criterion with the Tresca stress amplitude, the ASMEcriterion and the Findley criterion. In addition to the traditional, proportionalmethod based on maxmin stressvalues over the course of a cycle, an ASMEmethod is proposed and implemented. The ASMEmethod calculates stressvalues based on intervals, which may or not coincide with the proportionalmethod of assessing stresses throughout a cycle. Both the criteria and the two assessmentmethods were evaluated and compared with respect to usability and quality of predictions. The normal stress criterion yielded nonconservative predictions for both the carbon/low alloyed steels and the aluminium alloy 76ST61 included in the compiled fatigue database. The accuracy for brittle materials was however unprecedented. The ASMEcriterion without correction for mean stresses yielded an almost astonishing overall mean predicted value of 0.99. The standard deviation however was the highest for all criteria, indicating a high spread in predictions. These were chiefly
57
7. Conclusion caused by test data with nonzero mean stresses. For the Findley criterion evaluated with two diﬀerent values of k, the ASMEassessment method yielded a significant improvement in the quality of predictions. However, the ASMEmethod had no eﬀect on other criteria such as the normal stress criterion. This indicates that the ASMEmethod may have a positive eﬀect on other criteria, and deserves further evaluation. From a userfriendly point of view, the MisesSines criterion based on stress invariants is the least challenging. Even though the concept of the vonMises stress invariant is not valid for nonproportional loading, the criterion yielded relatively good predictions overall. The critical plane criteria, here represented by normal stress, TrescaSines and Findley all require computations to be done over a wide range of angles. Findley requiring the determination of at least the material parameter k is the least user friendly of the three. The computability is severely decreased when the criteria are assessed with the ASMEmethod. This is especially the case for criticalplane criteria. With the overall result of improved predictions, this is an aspect that needs to be considered. The overall conclusion of this thesis is that multiaxial fatigue assessment is an incredibly complex process. Knowledge in a variety of disciplines is necessary in order to eﬀectively perform a proper evaluation, and computational experience is a must. The benefit of performing such an analysis is the better predictability of fatigue failure.
58
Bibliography [1] J. A. Schmidt. The definition of structural engineering. http://www.structuremag.org/article.aspx?articleID=829, last checked: 13/12 2013. [2] I. V. Papadopoulos, P. Davoli, C. Gorla, M. Filippini, and A. Bernasconi. A comparative study of multiaxial highcycle fatigue criteria for metals. International Journal of Fatigue, 19(3):219–235, 1997. [3] A. Carpinteri and A. Spagnoli. Multiaxial highcycle fatigue criterion for hard metals. International Journal of Fatigue, 23(2):135 – 145, 2001. [4] J. O. Nøkleby. Fatigue under multiaxial stress conditions. PhD thesis, Division of Machine Elements, The Norwegian Institute of Technology, Trondheim, Norway., 1980. [5] J. Papuga. Pragtic website. http://www.pragtic.com/, last checked: 13/122013. [6] A. Troost, O. Akin, and F. Klubberg. Versuchsund rechendaten zur dauerschwingfestigkeit von metallischen werkstoﬀen unter mehrachsiger beanspruchung. Materialwissenschaft und Werkstoﬀtechnik, 23(1):1–12, 1992. [7] N. E. Dowling. Mechanical behavior of materials: engineering methods for deformation, fracture, and fatigue. Pearson, Boston, 4th ed edition, 2013. [8] D. F. Socie and G. B. Marquis. Multiaxial fatigue. Society of Automotive Engineers, Warrendale, Pa., 2000. [9] G. Härkegård. Fatigue assessment of engineering components subjected to arbitrary multiaxial stress histories, February 2013. [10] G. Sines, J. L. Waisman, and T. J. Dolan. Metal fatigue, pages 145–169. McGrawHill, 1959. [11] E. Roos. Festigkeitslehre 1. Institut für Materialprüfung, Werkstoﬀkunde und Festigkeitslehre, Universität Stuttgart, 34. auflage edition, 2010.
59
Bibliography [12] W. N. Findley. A theory for the eﬀect of mean stress on fatigue of metals under combined torsion and axial load or bending. Basic research on fatigue failures under combined stress: Technical report. Engineering Materials Research Laboratory, Division of Engineering, Brown University, 1958. [13] B. Crossland. Eﬀect of large hydrostatic pressures on the torsional fatigue strength of an alloy steel. In Proc. Int. Conf. on Fatigue of Metals, Institution of Mechanical Engineers, London, pages 138–149, 1956. [14] DL. McDiarmid. A shear stress based criticalplane criterion of multiaxial fatigue failure for design and life prediction. Fatigue & Fracture of Engineering Materials & Structures, 17(12):1475–1484, 1994. [15] DL. McDiarmid. A general criterion for high cycle multiaxial fatigue failure. Fatigue & Fracture of Engineering Materials & Structures, 14(4):429–453, 1991. [16] T. Matake. An explanation on fatigue limit under combined stress. Bulletin of JSME, 20(141):257–263, 1977. [17] W. Navidi. Statistics for Engineers and Scientists, pages 13–14. McGrawHill, second edition. [18] Rechnerischer Festigkeitsnachweis für Maschinenbauteile, page 87. VDMAVerlag, 6 edition, 2012. [19] Rechnerischer Festigkeitsnachweis für Maschinenbauteile, pages 96–97. VDMAVerlag, 6 edition, 2012. [20] H. J. Gough and H. V. Pollard. The strength of metals under combined alternating stresses. Proceedings of the Institution of Mechanical Engineers, 131(1):3– 103, 1935. [21] S. Lasserre and C. Froustey. Multiaxial fatigue of steel  testing out of phase and in blocks: validity and applicability of some criteria. International journal of fatigue, 14(2):113–120, 1992. [22] H. Zenner, R. Heidenreich, and I. Richter. Dauerschwingfestigkeit bei nichtsynchroner mehrachsiger beanspruchung. Materialwissenschaft und Werkstoﬀtechnik, 16(3):101–112, 1985. [23] A. Banvillet, T. PalinLuc, and S. Lasserre. A volumetric energy based high cycle multiaxial fatigue citerion. International journal of fatigue, 25(8):755–769, 2003. [24] C. Froustey and S. Lasserre. Multiaxial fatigue endurance of 30ncd16 steel. International Journal of Fatigue, 11(3):169 – 175, 1989.
60
Bibliography [25] H. J. Gough. Engineering steels under combined cyclic and static stresses. Proceedings of the Institution of Mechanical Engineers, 160(1):417–440, 1949. [26] W. N. Findley. Combinedstress fatigue strength of 76st61 aluminum alloy with superimposed mean stresses and corrections for yielding, 1953. [27] T. Nishihara and M. Kawamoto. The strength of metals under combined alternating bending and torsion with phase diﬀerence. Memories of the College of Engineering, Kyoto Imperial University, 11(85):112, 1945. [28] L. Issler. Festigkeitsverhalten metallischer Werkstoﬀe bei mehrachsiger phasenverschobener Schwingbeanspruchung. PhD thesis, Staatl. Materialprüfungsanst. TU Stuttgart, 1973. [29] E. ElMagd and S. Mielke. Dauerfestigkeit bei überlagerter zweiachsiger statischer beanspruchung. Konstruktion, 29(7):253–257, 1977. [30] A. Troost, E. ElMagd, and S. Keil. Grundlagen zur berechnung der schwingfestigkeit bei mehrachsiger beanspruchung ohne phasenverschiebung: Schwingfestigkeit ohne phasenverschiebung. Forschungsbericht des Landes NRW, Fachgruppe Maschinenbau/verfahrenstechnik, Westd. Verlag, Nr 2812, 1979. [31] F. J. Baier. Zeitund Dauerfestigkeit bei überlagerter statischer und schwingender Zug, Druckund Torsionsbeanspruchung. PhD thesis, Diss. Staatl. Materialprüfungsanst. TU Stuttgart, 1970. [32] A. Galtier. Contribution à l’étude de l’endommagement des aciers sous solicitations uni ou multiaxials. PhD thesis, ENSAM CER de Bordeaux, France, 1993. [33] R. Heidenreich. Schubspannungsintensitätshypothese  dauerschwingfestigkeit bei mehrachsiger beanspruchung. Forschungshefte FKM, Heft 105, 1983. [34] R. Heidenreich and H. Zenner. Schubspannungsintensitaetshypotheseerweiterung und experimentelle abschaetzung einer neuen festigkeitshypothese fuer schwingende beanspruchung. Forschungshefte FKM, (77), 1979. [35] H. Zenner and R. Heidenreich. Festigkeitshypothese  berechnung der dauerfestigkeit für beiliebige beanspruchungskombinationen. Forschungshefte FKM, Heft 55, 1979. [36] C. Froustey, S. Lasserre, and L. Dubar. Validité des critères de fatigue multiaxiale à l’endurance en flexiontorsion. MatTech, 92:79–82, 1992. [37] S. Mielke. Festigkeitsverhalten metallischer Werkstoﬀe unter zweiachsig schwingender Beanspruchung mit verschiedenen Spannungszeitverläufen. PhD thesis, Aachen, Techn. Hochsch., Fak. für Maschinenwesen„ 1980.
61
Bibliography [38] W. Lempp. Festigkeitsverhalten von Stählen bei mehrachsiger Dauerschwingbeanspruchung durch Normalspannungen mit überlagerten phasengleichen und phasenverschobenen Schubspannungen. PhD thesis, Staatl. Materialprüfungsanst., 1977. [39] F. Klubberg. Zweiachsige Schwingfestigkeitsversuche mit drei schwingenden Lastkomponenten und vergleichende Auswer tung nach verschiedenen statistischen Methoden. PhD thesis, RWTH Aachen, 1985. [40] A. Troost, O. Akin, and F. Klubberg. Dauerfestigkeitsverhalten metallischer werkstoﬀe bei zweiachsiger beanspruchung durch drei phasenverschoben schwingene lastspannungen. Konstruktion, 39:479–488, 1987. [41] P. Grün, A. Troost, O. Akin, and F. Klubberg. Langzeitund dauerschwingfestigkeit des vergütungsstahls 25crmo4 bei mehrachsiger beanspruchung durch drei schwingende lastspannungen. Materialwissenschaft und Werkstoﬀtechnik, 22(3):73–80, 1991. [42] T. PalinLuc. Fatigue multiaxiale d’une fonte GS sous sollicitations combinées d’amplitude variable. PhD thesis, ENSAM CER de Bordeaux, 1996. [43] M. Bennebach. Fatigue multiaxiale d’une fonte GS. Influence de l’entaille et d’un traitement de surface. PhD thesis, ENSAM CER de Bordeaux, 1993. [44] L. Susmel. La progettazione a fatica in presenza di stati complessi di sollecitazione. PhD thesis, Universita degli Studi di Padova, 2002.
62
List of Figures 2.1.1.3Dcoordinate system. . . . . . . . . . . . . . . . . . . . . . . . . . 2.1.2.Element showing stress components for plane stress, σz = 0. . . . . 2.2.1.Failure locus showing the fatigue limits for fully reversed stresses in shear and normal stress. . . . . . . . . . . . . . . . . . . . . . . . . 2.2.2.Haighdiagram. . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. .
6 8
. 9 . 10
4.8.1.Example of a failure assessment diagram for the TrescaSines criterion. 27 4.10.1. Cyclic stresses for dynamically loaded mechanical component. . . . . 31 5.2.1.Failure assessment diagram, R = −1 and αij = 0◦ . Test data are 34 fatigue tests for carbon/low alloy steels. . . . . . . . . . . . . . . . . 5.2.2.Failure assessment diagram, R = −1 and αij = 0◦ . Test data are 13 fatigue tests for 76ST61. . . . . . . . . . . . . . . . . . . . . . . . . 5.2.3.Failure assessment diagram, R = −1 and αij = 0◦ . Test data are 12 fatigue tests for cast irons. . . . . . . . . . . . . . . . . . . . . . . . 5.3.1.Predictions and their distribution for the criteria normal stress, MisesSines and TrescaSines for all 268 tests. . . . . . . . . . . . . . . . . 5.3.2.Histograms of all predictions from the ASME criterion and Findley k(σA ) and k(τW ) for 268 tests. . . . . . . . . . . . . . . . . . . . . . 5.4.1.Stresses throughout the cycle on critical planes predicted by the criticalplane criteria. . . . . . . . . . . . . . . . . . . . . . . . . . .
. 35 . 36 . 36 . 38 . 39 . 46
6.3.1.Stress cycle with one shear and one normal stress component. . . . . 51
63
List of Tables 2.1. Support factors for types of material groups according to FKMRichtlinie. 16 3.1. Given and calculated material parameters for carbon steels and alloyed steels. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18 3.2. Given and calculated material parameters for aluminium alloys and cast irons. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19 4.1. List of materials collected from the literature and their references. For some materials, several data sets exist and and each individual data set is numbered with a number inside a parenthesis. . . . . . . 30 4.2. Extreme values of stresses during a cycle of a dynamically loaded component. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 32 4.3. Material parameters for a constructed steel according to FKMRichtlinie and assumed to be valid for the stress cycle given in figure (4.10.1). . 32 5.1. Average values of M, k(σA ) and k(τW ) reported in table 3.1 and 3.2 with respect to material grouping. Only values used in the fatigue analysis was counted in. . . . . . . . . . . . . . . . . . . . . . . . . . 33 5.2. Comparison of predictions for all criteria and diﬀerent loading cases. The predictions are presented as the mean value plus/minus one standard deviation, mp ± sp . . . . . . . . . . . . . . . . . . . . . . . . 41
5.3. Comparison of predictions for all criteria, a selection of stress components present, and diﬀerent groups of materials. No selection of stressratios or the like have been made. The predictions are presented as the mean value plus/minus one standard deviation, mp ± sp . . 42 5.4. Results of stresscycle assessment for all criteria and both assessment methods normalized with σW . . . . . . . . . . . . . . . . . . . . . . . 44 5.5. Results of stresscycle assessment for all criteria and both assessment methods. The names for the criteria are shortened, so that NS corresponds to the normal stress criterion etc. . . . . . . . . . . . . . . 45
65
List of Tables A.1. Specimens, number of cycles the fatigue limits given in table 3.1 and 3.2 are valid for, and their method of determination. . . . . . . . . . . A.2. Data collected from Gough [25]. Material parameters given in table 3.1. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A.3. Data collected from Gough [25]. Material parameters given in table 3.1 and 3.2. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A.4. Data collected from Froustey [24, 21]. Material parameters given in table 3.1. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A.5. Data collected from Carpinteri [3]. Material parameters given in table 3.1 and 3.2. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A.6. Data collected from Zenner [22]. Material parameters given in table 3.1. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A.7. Data from collected from Zenner [22]. Material parameters given in table 3.1. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A.8. Data collected from Troost [6]. Material parameters given in table 3.1. A.9. Data collected from Troost [6]. Material parameters given in table 3.1 and 3.2. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A.10.Data from Findley [26]. Material parameters given in table 3.1. . . . . A.11.Data collected from Banvillet [23]. Material parameters given in table 3.1 and 3.2. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . B.1. B.2. B.3. B.4. B.5. B.6. B.7.
66
Predictions Predictions Predictions Predictions Predictions Predictions Predictions
for for for for for for for
all all all all all all all
tests tests tests tests tests tests tests
and and and and and and and
selected selected selected selected selected selected selected
criteria. criteria. criteria. criteria. criteria. criteria. criteria.
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
68 69 70 71 72 73 74 75 76 77 78 80 81 82 83 84 85 86
A. Material Data
67
A. Material Data
Table A.1.: Specimens, number of cycles the fatigue limits given in table 3.1 and 3.2 are valid for, and their method of determination. Material
Ref.
Spec. Nf
Determined by
Carbon and low alloy steels 0.1 % C Steel [25] XC18 Steel [21] Mild Steel [3] St35 Steel [22] St60 Steel [6] Swedish Hard Steel [3] Ck 35 V [6] C20 annealed Steel [23] 34Cr4 (1) [22] 34Cr4 (2) [22] 34Cr4 (3) [22] 30CrMo16 (1) [24, 21] 30CrMo16 (2) [23] 25CrMo4 (1) [21] 25CrMo4 (2) [22] S65A [25] 42CrMo4 [22] 25CrMo4 (3) [6] 3.5% NiCr steel [25] 34CrMo4 V [6]
SS SS HS HS SS HS SS HS SS SS SS SS HS HS SS HS HS SS SS
107 106 106 or more 2 · 106 2 · 106 106 or more 107 106 or more 1, 5 · 106 2 · 106 1, 5 · 106 106 106 or more 2 · 106 107 2 · 106 107 107 107
SN testing Staircase method, Staircase method, Staircase method Staircase method Staircase method SN testing Staircase method, Staircase method, Staircase method. SN testing SN testing 
Aluminium 76ST61 (1) 76ST61 (2) 76ST61 (3)
[26] [26] [26]
SS SS SS
106 107 108
SN testing SN testing SN testing
Nodular graphite cast irons “Silal” cast iron [20] ENGJS8002 [23]
SS 
107 106 or more
SN testing Staircase method, ≥15 spec.
Lamellar graphite cast irons GG30 [6] Cast iron [3]
SS SS
107 

1012 spec.
≥15 spec.
≥15 spec. ≥15 spec.
() Stress values are calculated for comparability but not used in later calculations. SS = Solid specimen, HS = Hollow specimen,  = No Info
68
Table A.2.: Data collected from Gough [25]. Material parameters given in table 3.1. σxa σxm σya σym τxya τxym αy αxy Nr. (MPa) (MPa) (MPa) (MPa) (MPa) (MPa) (◦ ) (◦ ) 0.1% C Steel from 1 268.7 2 262.5 3 242.4 4 205.4 5 146.7 6 78.7 7 0
Gough [25]. 0 0 0 0 0 0 0 0 0 0 0 0 0 0
S65A from Gough [25]. 152 552.9 266.4 153 532.8 532.8 154 0 0 155 0 0 156 549.8 0 157 540.5 0 158 556 266.4 159 556 266.4 160 469.5 532.8 161 472.6 532.8 162 0 266.4 163 0 532.8 164 0 266.4 165 0 532.8 166 0 266.4 167 0 532.8 168 547.5 0 169 389.2 0 170 168.3 0 171 496.5 266.4 172 374.5 266.4 173 161.4 266.4 174 428.6 532.8 175 315.1 532.8 176 126.6 532.8 177 386.1 266.4 178 383.8 0
0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0
0 0 0 0 0 0 0
0 35.5 69.5 103.4 126.6 146.7 151.3
0 0 0 0 0 0 0
0 0 0 0 0 0 0
0 0 0 0 0 0 0
0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0
0 0 339 343.6 0 0 0 0 0 0 312 284.2 304.3 281.1 308.9 293.4 156 259.5 335.9 141.3 249.4 322 121.2 210 251.7 257.1 255.6
0 0 169.9 343.6 169.9 343.6 169.9 343.6 169.9 343.6 0 0 169.9 169.9 343.6 343.6 0 0 0 169.9 169.9 169.9 343.6 343.6 343.6 0 169.9
0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0
0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0
69
A. Material Data
Table A.3.: Data collected from Gough [25]. Material parameters given in table 3.1 and 3.2. σxa σxm σya σym τxya τxym αy αxy Nr. (MPa) (MPa) (MPa) (MPa) (MPa) (MPa) (◦ ) (◦ )
70
3.5% NiCr Steel from Gough [25]. 200 540.4 0 0 201 538.9 0 0 202 491.0 0 0 203 410.7 0 0 204 328.9 0 0 205 179.1 0 0 206 0.0 0 0
0 0 0 0 0 0 0
0.0 71.0 142.0 205.4 284.1 333.5 352.0
0 0 0 0 0 0 0
0 0 0 0 0 0 0
0 0 0 0 0 0 0
“Silal” Cast Iron from Gough [25]. 243 240.9 0 0 244 234.7 0 0 245 210.0 0 0 246 194.5 0 0 247 152.9 0 0 248 89.6 0 0 249 0.0 0 0
0 0 0 0 0 0 0
0.0 30.9 60.2 97.3 132.8 166.8 219.2
0 0 0 0 0 0 0
0 0 0 0 0 0 0
0 0 0 0 0 0 0
Table A.4.: Data collected from Froustey [24, 21]. Material parameters given in table 3.1. σxa σxm σya σym τxya τxym αy αxy Nr. (MPa) (MPa) (MPa) (MPa) (MPa) (MPa) (◦ ) (◦ ) XC18 Steel from Froustey/Lasserre [21]. 8 310 0 0 0 9 0 0 0 0 10 230 0 0 0 11 230 0 0 0 12 242 0 0 0
0 179 133 133 140
0 0 0 0 0
0 0 0 0 0
0 0 0 45 90
30CrMo16 (1) from Froustey/Lasserre [24, 21]. 95 630 300 0 0 0 96 0 300 0 0 370 97 211 300 0 0 365 98 220 300 0 0 385 99 590 300 0 0 148 100 563 300 0 0 141 101 540 300 0 0 135 102 480 300 0 0 277 103 480 300 0 0 277 104 470 300 0 0 271 105 473 300 0 0 273 106 710 0 0 0 0 107 0 0 0 0 450 108 485 0 0 0 280 109 480 0 0 0 277 110 0 300 0 0 395
0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0
0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0
0 0 0 90 0 45 90 0 45 60 90 0 0 0 90 0
25CrMo4 (1) from 140 361 141 270 142 261 143 277
0 0 0 0
0 0 0 0
0 0 60 90
Mielke [37]. 0 0 0 0 0 0 0 0
0 0 0 0
0 135 131 139
71
A. Material Data
Table A.5.: Data collected from Carpinteri [3]. Material parameters given in table 3.1 and 3.2. σxa σxm σya σym τxya τxym αy αxy Nr. (MPa) (MPa) (MPa) (MPa) (MPa) (MPa) (◦ ) (◦ ) Mild steel from Nishihara/Kawamoto [27]. 13 245.3 0 0 0 14 235.6 0 0 0 15 187.3 0 0 0 16 101.3 0 0 0 17 0 0 0 0 18 194.2 0 0 0 19 108.9 0 0 0 20 235.6 0 0 0 21 208.1 0 0 0 22 112.6 0 0 0 Swedish 42 43 44 45 46 47 48 49 50 51 52 53
hard steel 327.7 308 255.1 141.9 0 255.1 142 255.1 147.2 308 264.9 152.5
from Nishihara/Kawamoto [27]. 0 0 0 0 0 0 0 63.9 0 0 0 127.5 0 0 0 171.3 0 0 0 201.1 0 0 0 127.5 0 0 0 171.2 0 0 0 127.5 0 0 0 177.6 0 0 0 63.9 0 0 0 132.4 0 0 0 184.2
Grey Cast Iron from Nishihara/Kawamoto 261 93.2 0 0 0 262 95.2 0 0 0 263 83.4 0 0 0 264 56.3 0 0 0 265 0 0 0 0 266 104.2 0 0 0 267 97.1 0 0 0 268 71.3 0 0 0
72
0 48.9 93.6 122.3 142.3 97.1 131.5 48.9 104.1 136
[27]. 0 19.7 41.6 68 94.2 21.6 48.6 86.1
0 0 0 0 0 0 0 0 0 0
0 0 0 0 0 0 0 0 0 0
0 0 0 0 0 60 60 90 90 90
0 0 0 0 0 0 0 0 0 0 0 0
0 0 0 0 0 0 0 0 0 0 0 0
0 0 0 0 0 30 30 60 60 90 90 90
0 0 0 0 0 0 0 0
0 0 0 0 0 0 0 0
0 0 0 0 0 90 90 90
Table A.6.: Data collected from Zenner [22]. Material parameters given in table 3.1. σxa σxm σya σym τxya τxym αy αxy Nr. (MPa) (MPa) (MPa) (MPa) (MPa) (MPa) (◦ ) (◦ ) St35 Steel from Issler [28]. 23 139 153 24 147 162 25 129 142 26 110 121 27 100 110 28 154 169 29 149 164 30 142 156 31 123 135 32 157 173 33 145 160 34 118 130
139 147 129 110 100 77 75 11 62 79 73 59
153 162 142 121 110 92 89 85 74 0 0 0
0 0 0 0 0 0 0 0 0 0 0 0
0 0 0 0 0 0 0 0 0 0 0 0
0 60 90 120 180 0 60 90 180 0 90 180
0 0 0 0 0 0 0 0 0 0 0 0
25CrMo4 (2) from Mielke 144 261 170 145 275 170 146 240 170 147 196 170 148 0 170 149 0 170 150 0 170 151 0 170
[37]. 261 275 240 196 220 233 155 159
340 340 340 340 340 340 340 340
0 0 0 0 110 117 155 159
0 0 0 0 0 0 0 0
0 60 90 180 0 0 0 0
0 0 0 0 60 90 60 90
0 0 0 0 0 0 0 0 0
157 137 224 205 134 130 128 136 160
0 0 0 0 0 0 128 136 160
0 0 0 0 0 0 0 0 0
0 90 0 90 0 90 0 90 180
42CrMo4 from Lempp [38]. 179 328 0 0 180 286 0 0 181 233 0 0 182 213 0 0 183 280 280 0 184 271 271 0 185 266 0 0 186 283 0 0 187 333 0 0
73
A. Material Data
Table A.7.: Data from collected from Zenner [22]. Material parameters given in table 3.1. σxa σxm σya σym τxya τxym αy αxy Nr. (MPa) (MPa) (MPa) (MPa) (MPa) (MPa) (◦ ) (◦ )
74
34Cr4 (1) from Heidenreich [33, 34, 35]. 68 225 275 225 275 69 225 275 225 275 70 190 232 190 232 71 205 250 205 250 72 175 214 175 214 73 181 221 181 221 74 195 238 195 238 75 192 234 192 234 76 180 220 180 220
0 0 0 96 82 85 92 90 85
0 0 0 0 0 85 92 90 85
0 60 180 0 180 0 0 60 180
0 0 0 0 0 0 90 90 90
34Cr4 (2) from Heidenreich [34, 35]. 77 314 0 0 0 78 315 0 0 0 79 316 0 0 0 80 315 0 0 0 81 224 0 0 0 82 380 0 0 0 83 316 0 0 0 84 314 0 0 0 85 315 0 0 0 86 279 279 0 0 87 284 284 0 0 88 355 0 0 0 89 212 212 0 0 90 129 0 0 0
157 158 158 158 224 95 158 157 158 140 142 89 212 258
0 0 0 0 0 0 158 157 158 0 0 178 0 0
0 0 0 0 0 0 0 0 0 0 0 0 0 0
0 60 90 120 90 90 0 60 90 0 90 0 90 90
34Cr4 (3) from Heidenreich [34, 35]. 91 280 0 0 0 92 309 0 0 0 93 320 160 0 0 94 350 175 0 0
140 155 160 175
280 309 160 175
0 0 0 0
0 180 0 180
Table A.8.: Data collected from Troost [6]. Material parameters given in table 3.1. σxa σxm σya σym τxya τxym αy αxy Nr. (MPa) (MPa) (MPa) (MPa) (MPa) (MPa) (◦ ) (◦ ) St60 Steel from El Magd/Troost [29].[30]. 35 290.4 0 0 306.8 36 259 0 0 460.2 37 286.5 76.7 0 306.8 38 259 76.7 0 460.2 39 280.6 153.4 0 153.4 40 278.6 153.4 0 306.8 41 262.9 153.4 0 460.2 Ck35 V Steel from Baier [31]. 54 273 0 0 55 273 0 0 56 216 0 0 57 229 229 0 58 181 181 0 59 0 0 0 60 0 547.75 0 61 0 275.44 0 62 0 294.22 0 63 0 441.33 0 64 0 588.44 0
0 0 0 0 0 0 0 0 0 0 0
25CrMo4 (3) from Klubberg/Troost/Grün 188 205 340 205.0 221 189 185 340 185.0 221 190 218.8 255 164.1 210.8 191 207.5 255 155.6 210.8 192 212.1 255 159.1 210.8 193 225 255 168.8 210.8 194 222.1 255 166.6 210.8 195 205 255 153.8 210.8 196 215 255 161.3 210.8 197 187.9 255 140.9 210.8 198 223.6 255 167.7 210.8 199 215 255 161.3 210.8
0 0 0 0 0 0 0
0 0 0 0 0 0 0
0 0 0 0 0 0 0
0 0 0 0 0 0 0
0 0 0 0 0 191 239 229 176 141 130
156.5 303.61 441.33 172.15 344.3 191 0 0 0 0 0
0 0 0 0 0 0 0 0 0 0 0
0 0 0 0 0 0 0 0 0 0 0
0 0 0 0 0 0 0 0 0 0 0 0
90 90 0 90 180 90 45 90 135 0 90 135
[39],[40],[41]. 102.5 0 92.5 0 109.4 0 103.75 0 106.05 0 112.5 0 111.05 0 102.5 0 107.5 0 93.95 0 111.8 0 107.5 88.4
75
A. Material Data
Table A.9.: Data collected from Troost [6]. Material parameters given in table 3.1 and 3.2. σxa σxm σya σym τxya τxym αy αxy Nr. (MPa) (MPa) (MPa) (MPa) (MPa) (MPa) (◦ ) (◦ )
76
34CrMo4 V from Baier [31]. 207 378 0 0 208 353 0 0 209 329 0 0 210 320 0 0 211 294 294 0 212 88 88 0 213 311 311 0 214 273 0 0 215 0 0 0 216 0 550.1 0 217 0 179.5 0 218 0 179.5 0 219 0 351.4 0 220 0 511.9 0 221 0 695.2 0
0 0 0 0 0 0 0 0 0 0 0 0 0 0 0
0 0 0 0 0 0 0 0 256 343 284 283 235 222 156
107.0 217.7 324.7 431.7 645.6 794.6 194.8 489.0 256 0 0 0 0 0 0
0 0 0 0 0 0 0 0 0 0 0 0 0 0 0
0 0 0 0 0 0 0 0 0 0 0 0 0 0 0
GG30 from Baier 254 145 255 127 256 107 257 99 258 96.5 259 75 260 53.5
0 0 0 0 0 0 0
0 0 0 0 0 0 0
74 112.5 146.5 186.5 108.0 217.6 196.8
0 0 0 0 0 0 0
0 0 0 0 0 0 0
[31]. 0 0 0 0 0 0 0
0 0 0 0 0 0 0
Table A.10.: Data from Findley [26]. Material parameters given in table 3.1. σxa σxm σya σym τxya τxym αy αxy Nr. (MPa) (MPa) (MPa) (MPa) (MPa) (MPa) (◦ ) (◦ ) 76ST61 (1) for 106 cycles. 222 217.9 0.0 223 0.0 0.0 224 215.8 0.0 225 171.0 0.0 226 153.1 82.7 227 129.6 206.8 228 139.3 0.0 229 104.5 0.0
0 0 0 0 0 0 0 0
0 0 0 0 0 0 0 0
0.0 143.4 44.7 85.5 76.5 64.8 101.9 126.2
0 0 0.0 0.0 41.4 103.4 0.0 0.0
0 0 0 0 0 0 0 0
0 0 0 0 0 0 0 0
76ST61 (2) for 107 cycles. 230 188.2 0.0 231 0.0 0.0 232 180.6 0.0 233 139.3 0.0 234 136.5 82.7 235 122.0 206.8 236 117.9 0.0 237 86.7 0.0
0 0 0 0 0 0 0 0
0 0 0 0 0 0 0 0
0.0 119.3 37.4 69.6 68.3 61.0 86.2 104.1
0.0 0 0.0 0.0 41.4 103.4 0.0 0.0
0 0 0 0 0 0 0 0
0 0 0 0 0 0 0 0
76ST61 (3) for 108 cycles. 238 170.3 0.0 239 0.0 0.0 240 124.8 0.0 241 12.4 82.7 242 102.7 0.0
0 0 0 0 0
0 0 0 0 0
0.0 109.6 62.4 62.1 75.2
0.0 0 0.0 41.4 0.0
0 0 0 0 0
0 0 0 0 0
77
A. Material Data Table A.11.: Data collected from Banvillet [23]. Material parameters given in table 3.1 and 3.2. σxa σxm σya σym τxya τxym αy αxy Nr. (MPa) (MPa) (MPa) (MPa) (MPa) (MPa) (◦ ) (◦ )
78
C20 annealed Steel from Galtier [32]. 65 246 0 0 0 66 246 0 0 0 67 264 0 0 0
138 138 148
0 0 0
0 0 0
0 45 90
30CrMo16 (2) from Froustey [36]. 111 575 375 0 112 558 428 0 113 627 273 0 114 679 156 0 115 519 0 0 116 514 0 0 117 451 294 0 118 462 294 0 119 474 294 0 120 464 294 0 121 554 287 0 122 474 0 0 123 220 199 0 124 470 299 0 125 527 287 0 126 433 472 0 127 418 622 0 128 0 299 0 129 0 486 0 130 0 655 0 131 482 0 0 132 207 299 0 133 474 294 0 134 584 281 0 135 447 473 0 136 425 635 0 137 235 745 0 138 251 704 0 139 527 222 0
0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0
0 0 0 0 291 288 250 258 265 259 135 265 368 261 129 240 234 396 411 364 268 350 265 142 252 223 0 0 0
0 0 0 0 0 0 191 191 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0
0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0
0 0 0 0 0 90 0 90 45 60 45 90 90 90 90 90 90 0 0 0 0 0 0 0 0 0 0 0 0
ENGJS8002 Cast Iron from [42],[43]. 250 228 0 0 0 251 245 0 0 0 252 199 0 0 0 253 184 225 0 0
132 142 147 0
0 0 0 0
0 0 0 0
0 90 0 0
B. Predictions
79
B. Predictions Table B.1.: Predictions for all tests and selected criteria. σar /σW Nr. Normal stress Findley (τW ) Findley (τW )ASME 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42
80
1.02 1.02 0.99 0.95 0.84 0.73 0.58 1.00 0.58 0.94 0.87 0.78 1.04 1.04 0.96 0.78 0.60 0.89 0.73 1.00 0.88 0.63 0.84 0.89 0.78 0.66 0.60 0.93 0.90 0.86 0.74 0.95 0.88 0.71 0.98 0.88 1.00 0.91 1.01 1.01 0.95 1.04
1.02 1.03 1.05 1.07 1.05 1.05 1.02 1.00 1.00 1.08 1.04 0.98 1.04 1.07 1.08 1.03 1.04 1.04 1.09 1.01 1.00 1.11 0.46 1.04 1.10 1.04 0.99 0.72 0.89 0.89 0.98 0.69 0.94 0.90 1.16 1.17 1.20 1.21 1.15 1.22 1.27 1.04
1.02 1.03 1.05 1.07 1.05 1.05 1.02 1.00 1.00 1.08 1.00 0.83 1.04 1.07 1.08 1.03 1.04 0.98 1.03 1.00 0.89 1.00 0.46 0.91 0.99 0.97 0.99 0.72 0.86 0.89 0.98 0.69 0.91 0.90 1.16 1.17 1.20 1.21 1.15 1.22 1.27 1.04
Table B.2.: Predictions for all tests and selected criteria. σar /σW Nr. Normal stress Findley (τW ) Findley (τW )ASME 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60 61 62 63 64 65 66 67 68 69 70 71 72 73 74 75 76 77 78 79 80 81 82 83 84
1.02 0.98 0.82 0.64 0.95 0.79 0.88 0.74 0.98 0.84 0.64 0.89 0.95 0.87 0.96 0.85 0.78 0.56 0.62 0.71 0.69 0.75 0.93 0.87 0.80 0.89 0.89 0.75 1.09 0.75 1.04 0.91 0.96 0.72 0.92 0.83 0.77 0.83 0.63 0.93 1.01 0.90
1.05 1.08 1.04 1.02 1.07 1.03 1.03 1.07 1.00 0.99 1.10 1.12 1.37 1.42 1.27 1.33 1.06 1.10 1.06 1.31 1.39 1.59 1.07 1.02 0.96 0.46 0.98 1.15 0.89 1.15 0.81 0.85 1.08 1.23 1.02 0.97 0.90 0.97 1.07 0.95 1.16 1.04
1.05 1.08 1.04 1.02 1.05 1.01 0.96 0.99 0.98 0.86 0.96 0.66 0.90 1.05 0.87 0.98 1.06 1.10 1.06 1.31 1.39 1.59 1.07 0.99 0.83 0.46 0.86 1.15 0.89 1.15 0.81 0.76 0.99 1.17 1.02 0.91 0.79 0.89 0.91 0.93 0.96 0.84
81
B. Predictions Table B.3.: Predictions for all tests and selected criteria. σar /σW Nr. Normal stress Findley (τW ) Findley (τW )ASME 85 86 87 88 89 90 91 92 93 94 95 96 97 98 99 100 101 102 103 104 105 106 107 108 109 110 111 112 113 114 115 116 117 118 119 120 121 122 123 124 125 126
82
0.80 0.99 0.89 0.98 0.70 0.65 0.97 0.77 0.93 0.82 1.09 0.63 0.83 0.69 1.08 1.02 0.96 1.04 0.98 0.92 0.86 1.08 0.68 0.93 0.73 0.67 1.01 1.01 1.04 1.06 0.94 0.74 0.99 0.82 0.92 0.87 0.96 0.69 0.61 0.82 0.90 0.85
0.99 1.16 1.09 1.12 1.21 1.10 1.14 1.18 1.12 1.07 1.07 1.08 1.17 1.22 1.13 1.06 0.96 1.20 1.18 1.14 1.10 1.08 1.10 1.05 0.94 1.14 0.97 0.97 1.01 1.04 1.06 0.94 1.05 1.03 1.09 1.05 0.99 0.87 1.07 1.02 0.89 1.05
0.74 1.16 0.95 0.83 1.06 1.02 0.80 0.96 0.81 0.95 1.07 1.08 1.17 1.13 1.13 1.05 0.94 1.20 1.13 1.06 0.93 1.08 1.10 1.05 0.77 1.14 0.97 0.97 1.01 1.04 1.06 0.78 1.03 0.85 1.06 0.99 0.98 0.72 0.98 0.87 0.87 0.91
Table B.4.: Predictions for all tests and selected criteria. σar /σW Nr. Normal stress Findley (τW ) Findley (τW )ASME 127 128 129 130 131 132 133 134 135 136 137 138 139 140 141 142 143 144 145 146 147 148 149 150 151 152 153 154 155 156 157 158 159 160 161 162 163 164 165 166 167 168
0.89 0.65 0.72 0.70 0.87 0.77 0.97 1.02 1.00 1.01 0.85 0.85 1.07 1.00 0.90 0.78 0.77 0.91 0.95 0.86 0.73 0.84 0.84 0.77 0.67 1.06 1.14 0.65 0.74 0.95 0.95 1.07 1.09 1.04 1.06 0.59 0.61 0.65 0.68 0.74 0.77 1.01
1.12 1.09 1.23 1.21 0.98 1.08 1.12 1.05 1.17 1.18 0.81 0.81 1.04 1.00 0.99 0.91 0.91 0.69 1.16 1.22 1.18 1.15 1.16 1.23 1.25 1.08 1.18 0.96 1.02 1.06 1.17 1.20 1.32 1.18 1.30 1.03 1.15 1.05 1.17 1.11 1.26 1.05
0.97 1.09 1.23 1.21 0.98 1.08 1.12 1.05 1.17 1.18 0.81 0.81 1.04 1.00 0.99 0.85 0.79 0.69 1.03 1.11 1.18 0.97 1.03 1.05 1.12 1.08 1.18 0.96 1.02 0.82 0.78 0.97 0.87 0.97 0.89 1.03 1.15 1.05 1.17 1.11 1.26 1.05
83
B. Predictions Table B.5.: Predictions for all tests and selected criteria. σar /σW Nr. Normal stress Findley (τW ) Findley (τW )ASME 169 170 171 172 173 174 175 176 177 178 179 180 181 182 183 184 185 186 187 188 189 190 191 192 193 194 195 196 197 198 199 200 201 202 203 204 205 206 207 208 209 210
84
0.89 0.74 1.06 1.00 0.85 1.08 1.02 0.84 0.97 0.94 0.98 0.72 0.93 0.60 1.01 0.87 0.87 0.73 0.93 0.85 0.68 0.99 0.73 0.96 0.80 0.86 0.71 0.81 0.72 0.76 0.79 1.00 1.01 0.98 0.92 0.91 0.80 0.65 0.99 0.94 0.90 0.91
1.02 1.00 1.15 1.13 1.16 1.25 1.16 1.17 1.20 1.10 1.07 0.84 1.11 1.00 1.22 1.11 1.00 0.94 1.19 1.38 1.34 1.16 1.12 1.14 1.29 1.29 1.28 1.30 1.24 1.35 1.40 1.00 1.02 1.02 1.00 1.07 1.06 1.00 1.15 1.27 1.38 1.53
1.02 1.00 1.05 1.13 1.16 1.05 1.16 1.17 1.20 0.96 1.07 0.74 1.11 0.84 1.22 0.98 0.81 0.68 0.92 1.25 1.28 1.16 0.98 1.08 1.13 1.14 1.10 1.17 1.24 1.27 1.24 1.00 1.02 1.02 1.00 1.07 1.06 1.00 0.84 0.78 0.90 1.06
Table B.6.: Predictions for all tests and selected criteria. σar /σW Nr. Normal stress Findley (τW ) Findley (τW )ASME 211 212 213 214 215 216 217 218 219 220 221 222 223 224 225 226 227 228 229 230 231 232 233 234 235 236 237 238 239 240 241 242 243 244 245 246 247 248 249 250 251 252
1.08 0.64 1.01 0.82 0.82 0.75 0.69 0.80 0.73 0.75 0.67 1.00 0.66 1.03 0.95 1.06 1.24 0.89 0.87 1.00 0.63 1.00 0.89 1.11 1.36 0.87 0.83 1.00 0.64 0.88 0.61 0.84 1.05 1.04 0.98 1.02 1.00 0.94 0.95 0.98 0.83 0.94
2.14 1.65 1.50 1.51 1.18 1.17 0.98 1.29 1.40 1.62 1.70 1.00 1.00 1.05 1.03 1.06 1.17 1.01 1.07 1.00 1.00 1.02 0.98 1.10 1.24 1.01 1.04 1.00 1.00 0.97 0.83 0.96 1.05 1.04 0.99 1.05 1.05 1.03 1.10 1.05 1.11 1.03
1.71 1.52 1.16 1.10 1.18 1.17 0.98 1.29 1.40 1.62 1.70 1.00 1.00 1.05 1.03 1.06 1.17 1.01 1.07 1.00 1.00 1.02 0.98 1.10 1.24 1.01 1.04 1.00 1.00 0.97 0.83 0.96 1.05 1.04 0.99 1.05 1.05 1.03 1.10 1.05 0.91 1.03
85
B. Predictions
Table B.7.: Predictions for all tests and selected criteria. σar /σW Nr. Normal stress Findley (τW ) Findley (τW )ASME
86
253 254 255 256 257 258 259 260 261 262 263 264 265 266 267 268
0.90 1.03 0.97 0.93 0.99 0.79 0.95 0.80 0.97 1.03 1.05 1.06 0.98 1.08 1.01 0.98
1.05 1.32 1.42 1.49 1.68 1.21 1.73 1.49 0.97 1.03 1.06 1.08 1.03 1.13 1.19 1.17
1.05 1.07 1.18 1.28 1.48 1.02 1.58 1.38 0.97 1.03 1.06 1.08 1.03 1.10 1.09 1.08
max min mp sp
1.36 0.56 0.88 0.14
2.14 0.46 1.10 0.18
1.71 0.46 1.03 0.17
View more...
Comments